In this brief review, we summarize and elaborate on some of the nomenclature of polaritonic phenomena and systems as they appear in the literature on quantum materials and quantum optics. Our summary includes at least 70 different types of polaritonic light–matter dressing effects. This summary also unravels a broad panorama of the physics and applications of polaritons. A constantly updated version of this review is available at https://infrared.cni.columbia.edu.
Polaritons are commonly described as light–matter hybrid quasiparticles. Polaritons inherit their attributes from both their light and matter constituents. More rigorously, a polariton is a quantum mechanical superposition of a photon with a matter excitation, the latter being a collective mode in solids and superconducting circuits or an electron in atoms, molecules or even superconducting qubits. As such, the notion of polaritons is a unifying universal concept between the fields of quantum materials (QMs) and quantum optics/electrodynamics. Until fairly recently, these subfields of contemporary physics evolved largely independently of each other. Among the unintended consequences of these divisions is the ambiguity in polaritonic terminology with the same terms used markedly differently in QMs and cavity quantum electrodynamics (QED) with atomic systems. Here, we attempt to summarize (in alphabetical order) some of the polaritonic nomenclature in the two subfields. We hope this summary will help readers to navigate through the vast literature in both of these fields . Apart from its utilitarian role, this summary presents a broad panorama of the physics and technology of polaritons transcending the specifics of particular polaritonic platforms (Boxes 1 and 2). We invite readers to consult with reviews covering many important aspects of the physics of polaritons in QMs , , , atomic and molecular systems , and in circuit QED , , as well as general reviews of the closely related topic of strong light–matter interaction , , , , , . A constantly updated version is available at https://infrared.cni.columbia.edu.
Anderson–Higgspolaritons , . The matter constituent of these polaritons originates from the amplitude mode in superconductors  (Figure 1). Anderson–Higgs polaritons are yet to be experimentally observed.
Bardasis–Schrieffer polaritons. The matter constituent of Bardasis–Schrieffer (BaSh) polaritons is associated with the fluctuations of subdominant order parameter in superconductors , , charge density wave systems , and excitonic insulators . This novel theoretical concept still awaits experimental confirmation. The requisite experiments include nanospectroscopy and nanoimaging of polaritonic dispersion in the terahertz (THz) frequency range below the energy gap of superconductors. These are challenging scanning probe measurements, as they have to be carried out at cryogenic temperatures. Nano-THz imaging at cryogenic temperatures have been recently fulfilled , paving the wave to the exploration of polaritonic phenomena in superconductors (see also Cooper pair plasmon polaritons and Josephson plasmon polaritons).
Berreman polaritons: Phonon polaritons in anisotropic materials and multilayer structures are also referred to as epsilon-near-zero or ENZ polaritons , , . ENZ materials, artificial structures, and nanocavities reveal exotic electromagnetic responses with a broad range of technological applications , , , , . For example, ENZ nanocavities facilitate ultrastrong coupling between plasmonic and phononic modes , as well as the so-called photonic doping .
Berry plasmon polaritons: chiral plasmonic modes whose dispersion is explicitly impacted by the Berry curvature and anomalous velocity in chiral media , , . Berry plasmon polaritons are yet to be experimentally observed.
Bose–Hubbard polaritons: cavity QED polaritons with matter component associated with transitions across the Mott gap in the system of interacting atoms  (see also Mott polaritons).
Bragg polaritons. Bragg reflectors (Box 1 panel G, Figures 2 and 4) are routinely utilized to implement polaritonic cavities. Bragg polaritons pertain to systems in which multiple excitonic layers and/or quantum wells are periodically integrated in a DBR cavity ,  (see also polaritonic lattices). The inherent anisotropy of Bragg multilayer structures may enable hyperbolic electrodynamics  (see hyperbolic polaritons).
Cavity (microcavity) polaritons. Weisbuch et al. devised and implemented the first semiconductor (micro)cavity device revealing Rabi splitting of exciton polaritons (Boxes 1 and 2). Semiconductor microcavites emerged as a powerful platform for the investigation of strong light–matter interaction in semiconductors , . Microcavity structures reveal intriguing phenomena including polariton parametric amplification  and its spontaneous counterpart, the parametric photoluminescence . Parametric photoluminescence is a purely quantum process. An appealing attribute of polariton parametric photoluminescence is that signal-idler polariton pairs are produced in nonclassical states with quantum correlations. The quest for Bose–Einstein condensation of microcavity polaritons has produced a stream of breakthrough results ,  (see also exciton polaritons and their condensates). Microcavity exciton polaritons display quantum effects including entanglement  and polariton blockade ,  and may serve as a platform for the implementation of qubits .
Channel polaritons are supported by materials and structures with a straight channel cut in polaritonic medium . Channel polaritons were utilized for the implementation of waveguide components including interferometers and ring resonators . Polaritons guided along the nanoslit are predicted to form hybrid polaritons, giving rise to both bonding and antibonding modes .
Charge transfer polaritons. The formation of plasmon polaritons in graphene or semiconductors relies on the high carrier density that can be introduced by electrostatic gating , , ferroelectric polarization , chemical doping , or photoexcitation . Alternatively, the requisite carrier density can be introduced by charge transfer across the interface between proximal materials with dissimilar work functions. Such charge transfer plasmon polaritons have been demonstrated for graphene residing on another van der Waals material RuCl3 . Experiments on metallic nanoparticles show that charge transmitted between the pair of nanoparticles through a conducting pathway leads to a characteristic plasmonic response  termed charge transfer plasmons. Interlayer exciton in transition metal dichalcogenide (TMDC) heterostructures (e.g., MoSe2/WSe2) also involves charge transfer from one layer to another; the relevant microcavity polaritons  are classified as charge transfer exciton polaritons.
Charged polariton. Charged polaritons posess a nonvanishing electric charge. This interesting concept was introduced in the context of the cavity exciton polaritons in GaAs/AlAs quantum wells that also hosted two-dimensional electron gas with the density ne. Spectroscopic experiments in a study by Forg et al.  have identified several distinct properties of charged exciton polaritons, including the scaling of the coupling strength analogous to the properties of atomic QED system . The effective mass of charged polaritons exceeds the band mass of a GaAs quantum well by a factor of 200. Tiene et al.  have theoretically demonstrated the unique utility of charged microcavity polaritons for exploring the physics of electron–hole systems with charge imbalance, which are difficult to access with alternative experimental methods. They demonstrated how the Fermi sea of excess charges modifies both the exciton properties and the dielectric constant of the cavity medium, which in turn affects the photon component of the many-body polariton ground state (Figure 2). See also the closely related entries of Fermi-edge exciton polaritons and trion polaritons.
Cherenkov polaritons. In the Cherenkov effect , a charged particle moving with a velocity faster than the phase velocity of light in the medium radiates light. The emitted radiation forms a cone with a half angle determined by the ratio of the two velocities. Genevet et al.  demonstrated that by creating a running wave of polarization along a one-dimensional metallic nanostructure consisting of subwavelength-spaced rotated apertures that propagates faster than the surface plasmon polariton phase velocity, one can generate surface plasmon wakes that serve as a two-dimensional analog of Cherenkov radiation. The Cherenkov physics is also relevant to the properties of phonon polaritons , . Infrared nanoimaging experiments reveal Cherenkov phonon polariton wakes emitted by superluminal one-dimensional plasmon polaritons in a silver nanowire on the surface of hexagonal boron nitride . See also Exciton polariton X-waves on superluminal properties in the system of exciton polaritons.
Cooper pairs polaritons (in QMs and cold fermionic cavity systems). Cooper pair plasmon polaritons emerge in superconductors. The matter component of these polaritons is associated with the superfluid density (from a study by Basov et al. ). The dispersion of Cooper pairs plasmon polaritons in layered cuprate high-Tc superconductors has been investigated theoretically ,  but is yet to be explored in experiments. Recently, the formalism of the Bardeen Cooper and Schrieffer theory of superconductivity has been applied to describe the quasiparticle excitations of a cold fermion system coupled to a cavity. Depending on the excitation density and atomic interaction, the excited atoms and holes and in the Fermi sea may form bound Cooper pairs strongly coupled with cavity photons. This latter kind of polaritons were also termed Cooper pair polaritons .
Dark polaritons in QMs: polaritons are characterized by a wavevector that lies beyond the light line. The lower branches of polaritons in many/most QM systems are dark by this criterion and do not couple to free space photons because of the notorious “momentum mismatch” problem (Box 1 F, H, Figure 1). Light excition of dark polaritons can be mediated by nanoscale defects such as a protrusions, divots, or cracks, exploiting the high spatial frequencies inherent to these deeply subwavelength objects. Better controlled strategies can also provide the missing momentum needed for coupling to dark polartons . These include prism and grating coupling, and the use of plasmonic optical nanoantennas , , , , , , , . Notably, sharp scan probe tips can act as such antennas , , , , , , allowing polaritonic waves to be launched and visualized. Scanning probe antenna-based nano-optics has emerged as an indespensible research tool enabling spectroscopy and visualization of polaritons in QMs , , .
Dark-state polaritons in atomic ensembles: typically, this refers to polaritons in atomic ensembles that propagate in the regime of electromagnetically induced transparency (EIT) , , , . The darkness arises from the photon mixing strongly with a collective atomic excitation, resulting in a state with only a minute photonic component. See also EIT polaritons below. In ordered atomic arrays, dark (also often referred to as subradiant) states emerge due to interference in photon emission and absorption. At the single photon level, these darks states are collective spin excitations with a wave vector that lies beyond the light line, preventing the coupling with radiation modes (exactly the same phenomenon of “momentum mismatch” described above for QMs) , , , . Polaritons arising in atomic lattices have applications in quantum information storage and processing .
Demons: or density modes were introduced by David Pines , an early protagonist of plasmons research. Demons are particularly relevant to the response of the Dirac fluid in graphene in hydrodynamic regime  and adiabatic plasmon amplification .
Dirac plasmon polaritons are formed by hybrids of infrared photons with Dirac electrons in graphene , , , . Direct nanoimaging experiments uncovered extraordinarily long propagation lengths of highly confined Dirac polaritons and have established fundamental limits underlying their decoherence and losses .
Dyakonov surface polaritons: the surface modes that propagate along the interface between isotropic and uniaxial materials is known as Dyakonov surface polaritons , , . A special case of Dyakonov polaritons is realized in anisotropic crystals of layered van der Waals materials. One example is that of the hyperbolic surface phonon polaritons propagating along the edges of slabs prepared from hexagonal boron nitride , , .
Edge magneto plasmons. Two-dimensional (2D) electron gas subjected to the magnetic field normal to the plane of the 2D conductors reveals two distinct field-dependent resonances: the cyclotron resonance mode with frequency increasing with the magnetic field and another mode that redshifts with the applied field. The latter mode has been linked to the edge plasmons of the charged sheet and can be viewed as the 2D analog of surface plasmons in three-dimensional (3D) systems . Specifically, edge magneto plasmons can propagate along the physical boundary of the 2D conductors , . Edge magneto plasmons constitute a spectacular manifestation of the dynamical Hall effect. Edge magneto plasmons are chiral. Their chirality is a direct implication of the applied Lorentz force . Graphene reveals rich plasmonic phenomena in the presence of magnetic fields , , , , .
Edge plasmon polaritons: one-dimensional plasmonic modes propagating along the physical boundaries of two-dimensional materials (Figure 3) is called edge plasmon polaritons. They reveal an approximately 10% shorter wavelength compared to the interior of the plasmonic medium . Qualitatively, the shorter wavelength can be ascribed to the effective reduction of the Drude weight since free carriers exist only on one side of the physical boundary. Dyakonov hyperbolic phonon polaritons are a lattice analog of edge plasmon polaritons. Berini reported on an in-depth numerical analysis of edge and corner plasmon polariton modes in thin conducting slabs . Whispering-galley polaritons is a special example of an edge polaritons that loops around the ridge of polartonic medium  or along the circumference of nanoholes , .
EIT in nanoplasmonic structures , , EIT with plasmon polaritons in graphene ,  and EIT with exciton polaritons in microcavities .
EIT polaritons propagate in atomic systems under conditions of EIT. A remarkable aspect of EIT polaritons is that they can be slowed down to 10s of meters per second  or even brought to a standstill , . EIT polaritons can be dark (decoupled from radiation, more “atom-like”) or bright (coupled to radiation, more “photon-like”). The darkness/brightness of the polaritons is controlled by an external laser beam. EIT polaritons can be strongly interacting, if coupled to Rydberg states (see Rydberg polaritons below). The EIT phenomenon is also observed in materials and nanostructures. Examples include:
ENZ polaritons: epsilon-near-zero or ENZ polaritons are equivalent to Berreman polaritons above.
Exciton polaritons and their condensates. Exciton polaritons are bosonic quasiparticles originating from photons hybridized with hydrogen-like bound electron–hole pairs. Semiconductor microcavities (Box 1 and Figure 4A) offer an outstanding platform for the investigation of exciton polaritons and the attendant strong light–matter coupling, provided a high-quality microcavity is nearly resonant with an excitonic transition. Trapped photons may be emitted and reabsorbed multiple times before being lost to dissipation or cavity leakage. Absorption and re-emission of photons in the cavity give rise to light–matter mixed eigenstates . When sufficiently long-lived, exciton polaritons may form coherent quantum states , , , , , , . Bose–Einstein condensates (BECs) of exciton polaritons are appealing quantum liquids in part because their coherent state is created and controlled by light , , . The binding energies of excitons in organic molecules , TMDCs, and lead halide perovskites can be as high as 0.75 eV , , , , , , , , ; these extraordinary high binding energies underlie the theoretical predictions of condensation and superfluidity at T = 300 K , , . BECs of exciton polaritons were predicted to form spatially and temporarily ordered states: time crystals . Exciton polariton condensates may also enable energy-efficient lasers .
Exciton polariton X-waves: wavepackets of exciton polaritons that sustain their shape without spreading, even in the linear regime. In a study by Gianfrate et al. . Self-generation of an X-wave out of a Gaussian excitation spot is obtained via a weakly nonlinear asymmetric process with respect to two directions of the nonparabolic polariton dispersion. Notably, X-waves were found to propage with supluminal peak speed with respect to the group velocity of the polaritonic system.
Fermi edge exciton polaritons ,  are observed in microcavities where the active semiconductor is heavily doped to form the Fermi edge. Fermi edge exciton polaritons are formed of electron hole pair excitations involving electron and hole states with in-plane wave vectors around the Fermi edge: kIIe = kIIh ∼ kF, where kF is the Fermi wavevector. In some literature, this latter form of polaritonic states are referred to Mahan exciton polaritons , recognizing a prediction of excitonic bound states in doped semiconductors beyond the critical density of the insulator to metal transition states by Mahan , . See also Quantum Hall polaritons below.
Floquet polaritons. The concept of Floquet engineering refers to the control of a system using a time periodic optical field and is being broadly applied in atomic physics, as well as in the field of QMs . The notion of Floquet polaritons pertains to polaritons in a system of Floquet-engineered atomic states  or electronic states in solids . The concept of Floquet engineering by time period optical fields has been extended to coherent phonons in QMs . Chiral Floquet polaritons are predicted  to form in chiral cavities, in which fundamental matter symmetries are broken (Box 2).
Frenkel exciton polaritons. The matter constituent of these polaritons originates from Frenkel excitons characterized by the Bohr radii of the same order as the size of the unit cell. Frenkel exciton polaritons are common in organic semiconductors . The high exciton binding energy (∼eV) and large oscillator strength may lead to room temperature exciton polariton condensates , , .
Fuchs–Kliewer interface polaritons: phonon polaritons occurring at surfaces and interfaces  with the matter part are originating from Fuchs–Kliewer surface phonons . Huber et al.  employed nanoinfrared methods to visualize propagating Fuchs–Kliewer surface phonon polaritons in SiC. Surface phonon polaritons are observed in insulating and semiconducting materials including hBN , , SiC , , , , GaAs , and many others.
Helical plasmon polaritons: were predicted to form in topologically nontrivial Weyl semimetals . Plasmon polariton dispersion may enable the detection of a chiral anomaly: a charge imbalance between the Weyl nodes in the presence of electric and magnetic fields . The Fermi surface of Weyl semimental features open disjoint segments – the Fermi arcs – associated with the topolical surface states. The resulting Fermi arc plasmon polaritons are predicted to be chiral and to reveal unidirectional propagation . Helical plasmon terminology was also applied to describe one-dimensional plasmon polaritons associated with the helical state in domain walls of topologically nontrivial conductors including anomalous quantum Hall systems . Helicity dependence of plasmon polaritons is discussed in the context of unidirectional propagation in plasmonic metastructures controlled by the circular polarization of light , .
Hopfield polaritons: a bold theoretical concept of light–matter hybridization proposed by John Hopfield in his doctoral thesis back in 1958 (in a study by Hopfield ). Hopfield also coauthored the first experimental paper on polaritons devoted to the study of phonon polariton dispersion in GaP by means of Raman scattering . Other early contributions to the theory of polaritons (short of introducing this term) were made by Fano , Huang , and Tolpygo .
Hybrid polaritons. Different types of polaritons hosted by the same material are prone to hybridization . For example, intersubband polaritons and phonon polaritons hybridize in semiconductor quantum wells , , . Hybridization can also occur in multilayered structures. In all-dielectric layered structures, phonon polaritons associated with the neighboring layers couple to form hybrid modes , , . Semiconductor heterostructures ,  and especially van der Waals heterostructures offer a fertile platform for the implementation of hybrid polaritons , . One such example (Figure 5B and C) is graphene surrounded by insulating layers of hexagonal boron nitride hBN or silicon dioxide. Plasmons associated with graphene layers hybridize with phonon polaritons in proximal SiO2 or hBN layers to form plasmon–phonon polaritons , , , . Hybrid polaritons at the interface of graphene with high-Tc superconductors were proposed as a tool to probe Anderson–Higgs electrodynamics . Hybrid polariton at the interface of graphene with a charge density wave materials were theoretically proposed to “melt” the density wave order . Hybrid modes produced by plasmons in graphene and molecular vibrations of absorbates on the graphene surface may enable high-selectivity sensing mechanisms , . A special case of hybrid modes is hybrid longitudinal–transverse phonon polaritons . Polaritonic heterostructures with phase change materials enable persistent switching of polaritonic response under thermal and optical stimuli .
Hyperbolic polaritons. Anisotropic media are predicted to support an interesting class of polaritonic light–matter modes referred to as “hyperbolic” because their isofrequency surface is a hyperboloid , , , , , , , , . These modes exist over a range of frequencies where the in-plane permittivity and the out-of-plane (c-axis) permittivity are of the opposite sign. Hyperbolic electrodynamics and hyperbolic polaritons can originate from a variety of physical processes including phonons , , , , , , , , , , ,  intersubband transitions in quantum wells , ,  plasmons , , , , , , excitons , and Cooper pairs (see Cooper pair polaritons). Hyperbolic polaritons dramatically enhance the local photonic density of states and are predicted to give rise to strong nonlinearities . Hyperbolic polaritons enable canalization imaging  with image effectively transferred by high-momentum subdiffractional polaritonic rays from back to front surface of the polaritonic medium , , , .
Image polaritons: virtual polariton modes produced by image charges at the interface of a polaritonic medium and a metal are called image polaritons. Lee et al.  have experimentally demonstrated low loss response of image polaritons at the interface of hBN separated with a thin spacer from a metallic substrate (Figure 5D).
Interband polaritons. The matter constituent of these polaritons originates from contributions of the optical response associated with transitions across the energy gap in the electronic spectrum of a material. These include transitions across the energy gap in semiconductors  and superconductors or transitions involving minibands/flat bands in moire superlattices of van der Waals materials , , ,  (see also Moire polaritons). The frequency dependence of σ2(ω)xω, where σ2(ω) is the imaginary part of the complex conductivity, is informative for the analysis of interband polaritons , . Spectra of σ2(ω)xω reveal a series of steps separated by plateaus, with each step uncovering the energy scale associated with separate interband contributions. In the limit of ω → 0, the product σ2(ω)xω quantifies the spectral weight of intraband processes to the plasmon polaritons. Interband effects play a central role in theoretical proposals for the implementation of population inversion , gain and superluminal plasmon polaritons .
Intersubband polaritons. Dini et al. ,  reported the first experimental observation of the vacuum-field Rabi splitting of an intersubband transition inside a planar microcavity hosting two-dimensional electron gas. Nonlinearities associated with intesubband transitions in semiconductors can be dramatically enhanced by in hybrid structure with plasmonic metasurfaces  (see also hybrid polaritons).
Josephson plasmon polariton: an inherent attribute of strongly anisotropic layered superconductors is the Josephson plasmon polariton. The matter constituent of Josephson plasmon polaritons originates from interlayer Josephson plasmon in layered superconducting materials such as cuprates , . Josephson plasmons are the electromagnetic signature of three-dimensional superconductivity in highly anisotropic layered high-Tc superconductors . Josephson plasma waves can be parametrically amplified under illumination with pulsed THz fields , paving the way for active Josephson polaritonics.
Kane polaritons: surface plasmon polaritons formed with Kane quasiparticles is the Kane polaritons. Kane polaritons were recently observed in pump–probe experiments on narrow gap II–VI semiconductors .
Landau polaritons. The matter component of Landau polaritons originates from cyclotron resonances and transitions between quantized Landau levels relevant in low-dimensional electron gases subjected to high magnetic fields , . See also magneto plasmon polariton.
Luttinger liquid polaritons: plasmon polaritons in one-dimensional conductors recently revealed by infrared nanoimaging of single-wall and multiple-wall carbon nanotubes . Interacting electrons confined in one dimension are generally described by the Luttinger liquid formalism , . Anomalous dependence of the plasmonic quality factor on gate voltage was interpreted in terms of plasmon–plasmon interaction in carbon nanotubes .
Magnon polaritons. The matter constituent of these polaritons originate from antiferromagnetic ,  and ferromagnetic resonances . In weak magnetic fields, surface magnon polaritons are predicted to acquire nonreciprocal properties. Macedo and Camley  analyzed the propagation of surface magnon polaritons in anisotropic antiferromagnets. Sloan et al.  predicted that surface magnon polaritons will strongly enhance the spin relaxation of quantum emitters in the proximity of antiferromagnetic materials such as MnF2 or FeF2. Kruk et al.  developed artificial structures with hyperbolic magnetic response with principal components of the magnetic permeability tensor having the opposite signs. Magnetic materials also support hybrid polaritons, including hybrid magnon–phonon polaritons recently observed in ErFeO3/LiNbO3 multilayers .
Magneto plasmon polaritons: coupled modes of magneto plasmons and THz/infrared photons , . Theoretically predicted unconventional properties of magneto polaritons in Weyl semimetals include hyperbolic dispersion and photonic stop bands . The nanoinfrared imaging and visualization of magneto plasmon polaritons remains an unresolved experimental challenge. Once technical obstacles are circumvented, it may become possible to directly explore both the focusing and the nonreciprocity predicted for magneto plasmon polaritons . Plasmonic system driven by intense a.c. field is predicted to reveal spontaneous symmetry breaking and nonlinear magnetism .
Microcavity polaritons: see cavity polaritons.
Moire polaritons. Atomic layers comprising van der Waals materials can be reassembled into heterostructures with nearly perfect interfaces , , . A unique control knob specific to vdW systems is the twist angle θ between the adjacent layers. Varying θ forms moiré superlattices that can radically modify the electronic structure and attendant properties , , , , , , , , , , , , , , . Plasmons, phonons, and excitons are all altered in moire superlattices prompting changes of the corresponding polaritons. G/hBN[cross-Ni-Moire]. Infrared nanoimaging data display rich real space patterns of polaritonis with selected examples of moire polaritons displayed in Figure 6. Morie design principle can be applied to epitaxially grown thin films on dielectric substrates . Recent experiments on interlayer excitons in TMDC heterobilayers have revealed the trapping of these excitons on the moire potential landscape , , , . When placed in an optical cavity, such moire trapped excitons may form an exciton polariton lattice and serve as analog quantum simulators (QSs) (see polaritonic lattices and quantum simulators).
Molecular polaritons. Organic semiconductors and molecules embedded in optical (nano)cavities under strong and ultrastrong coupling promote the dynamical formation of molecular polaritons: hybrid energy eigenstates composed of entangled photonic, electronic, and vibrational degrees of freedom , , . Molecular polaritons were demonstrated to enhance energy transfer  and DC conductivity . Progress with nanostructures enabled a demonstration of the strong–light matter coupling with a single molecule embedded in a plasmonic cavity . Molecular molaritons enable control of optical nonlinarities via manipulations of cavity characteristics . Molecular polaritons can form hybrid polaritons by coupling to surface plasmons , for example. We remark that molecular polaritons are commonly referred to as vibrational polaritons.
Mott polaritons (QED): nonequilibrium driven states in an array of circuit QED cavities or optical resonators ,  is the Mott polaritons. See also polaritonic lattices.
Mott polaritons (QM) were also introduced in context of the resonant coupling between strongly correlated electrons in solid Mott insulators integrated in a single-mode cavity .
Phonon polaritons: is a collective excitation comprised (infrared) light coupled with a polar lattice vibration. Like other polaritons, phonon polaritons can be understood in terms of an anticrossing of the dispersion curves of light and matter constituents (Figure 5). Early observations of phonon polaritons (see Hopfield polaritons) in bulk crystals and films were made using a variety of spectroscopic methods , . More recent work  has focused on the generation, detection, and on picosecond polaritons dynamics , , , , . By matching the phonon polariton velocity in LiNbO3 crystal to the group velocity of the fs punp pulse Yeh et al.  have been able to generate intense THz fields of the order of 10 μJ energy. Advanced nanoimaging/spectroscopy methods , ,  were employed for the real-space visualization of phonon polariton standing ways. Phonon polaritons play a major role in nanoscale thermal transport at nanoscale and mesoscale , , , , , , . Phonon polaritons in the anisotropic oxide material MoO3 reveal both elliptical and hyperbolic dispersions , , . The dispersion and propagation of phonon polaritons can be controlled by nanostructuring  and twist-angle (moire) engineering (Figure 6). The recent discovery of parametric phonon amplification in SiC paves the way for the exploration of nonlinear and active phonon polariton phenomena . Surface phonon polaritons (see also Fuchs–Kliewer interface polaritons) reveal a dispersion branch located between longitudinal and transverse vibrational modes (see hybrid polaritons). Dai et al.  detected surface phonon polaritons in monolayers of hBN.
Plasmon polaritons: probably the most thoroughly studied class of polaritons. A surface plasmon polariton is a transverse magnetic (TM)-polarized optical surface wave that, for example, propagates along a flat metal–dielectric interface, typically at visible or infrared wavelengths , , . Plasmon polaritons have rich implications for technology , , , . Nonlinear , ,  and quantum , , , ,  properties of plasmonic structures are in the vanguard of current research. Plasmon polaritons can be controlled at femto-second timescales , , , , ,  enabling access to novel physics and applications , . Plasmonic waveguides have been incorporated with light-emitting materials, paving the way for integrated plasmonic and photonic structures . Plasmon polaritons have been harnessed to implement high-quality factors such as whispering gallery microcavities . In parallel, many research groups are searching for new plasmonic media with the properties optimized for different classes of plasmonic effects , , , . Van der Waals materials, and especially graphene, are emerging as outstanding plasmonic media in light of their inherent tunability with different stimuli (see Dirac plasmons). Acoustic plasmon polaritons are a special example of hybrid polaritons whose frequency-momentum ω(q) dispersion is predicted to be linear , , , , . Acoustic plasmon plaritons have been demonstrated , ,  in structures, where graphene resides in close proximity to metallic surfaces. Spoof surface plasmons polaritons were introduced describe plasmon polaritons on the surface of artificial metallic structures and metamaterials . Airy surface plasmon polaritons are the surface counterparts of nondiffracting airy waves  and have been demonstrated by direct nanoimaging . Chiral plasmon polaritons  were predicted to occur in twisted bilayer graphene  (Figure 7).
Plexcitons are a specific example of hybrid polaritons. The matter constituent of plexcitons originates from plasmon exciton coupled modes , , , , , ,  Historically, plexciton studies have focused primarily on localized states , . Propagating plexciton states also exist and offer potential for compact quantum information carriers as well as opportunities for mediating emitter–emitter coupling , , . Composite structures and multilayers can feature plexcitons. An interesting recent example of plexciton study has been conducted in the setting of scanning probe nano-optical imaging and spectroscopy (Figure 8). This work by May et al. , along with a study by Groß et al. , implemented the scanning optical cavities formed between a nano-optical antenna and the substrate. The authors investigated CdSe/ZnS quantum dots using this scanning cavity approach and observed plexitonic Rabi splitting of 163 meV.
Polaritons parametric amplification, gain, and lasing have been demonstrated for exciton polaritons in microcavities , , , . Resonant coupling between photons and excitons in microcavities can efficiently generate significant single-pass optical gains . Polaritonic lasing has been implemented and analyzed in different material systems hosting plasmon polartions and exciton polaritons . Amplification of demons  has been predicted as well but is yet to be experimentally demonstrated.
Polaritonic chemistry: an emerging field focused on modifying pathways of chemical reactions in molecular systems coupled to photonic cavities , , , , .
Polaritonic circuits, devices, arrays, and systems. Both light and matter constituents of polaritons are amenable to controls with external stimuli . The use of exciton polaritons as building blocks for future information processing such as spin switches , spin memory , transistors , logic gates , resonant tunneling diodes , routers , and lasers  has recently been demonstrated. The first polaritonic systems are also emerging and include QSs and networks for neuromorphic computers . TMDC material WSe2 integrated into microcavity devices acts as efficient light emitting device .
Polaritonic lattices, and QSs. A variety of experimental approaches have been utilized to implement one- and two-dimensional arrays of interacting polaritons. In the field of microcavity exciton polaritons gate arrays, spatially dependent optical potential as well as surface acoustic waves , have been utilized to generate arrays/lattices . One-dimensional exciton polariton superlattices reveal weak lasing assigned to a novel type of a phase transition in this interacting system . Arrays of evanescently coupled cavities hosting neutral atoms  have been proposed as QSs, where the photon blockade provided by the atom limits the occupancy of each cavity to one, allowing for the implementation of the Bose–Hubbard model. QSs require controllable quantum systems that efficiently simulate a Hamiltonian of interest, which may encode phases with a significant degree of entanglement and is not amenable to calculations by classical computer , , , , , . Lattices of exciton polaritons , , , , ,  have emerged as a promising platform for QS, along with ultracold atoms , , trapped ions , , , and superconducting circuits , . Moire superlattices of plasmon polaritons (Figure 6) present yet another example of polaritonic lattices. Moire superlattices were realized in graphene devices with nanostructured gate electrodes , as well as in moire superlattices of twisted graphene layers .
Polaritonic interference, refraction, collimation, front shaping, and waveguiding. All these common wave phenomena are relevant to polaritons (Figure 9). In van der Waals materials, domain wall boundaries can act a polaritonc reflectors , , , or conductors . Zia and Brongersma  demonstrated Young’s double-slit experiments with surface plasmon polaritonss. Beyond analogs of geometrical optics effects, polaritons offer at least two novel routes for image formation. First, hyperbolic polaritons enable canalization imaging , with images effectively transferred by high-momentum subdiffractional polaritonic rays from the back to the front surface of the polaritonic medium , , ,  (Figure 9C). Second, polaritons are amenable to guiding and steering using methods of transformation optics. Polaritonic waveguides have been implemented over a broad range of frequencies from THz  and infrared regions to visible light. Peier et al. observed phonon–polariton tunneling across the airgap . Advanced polaritonic launchers and metalenses (Figure 9D) are well suited for defining the trajectories of polaritonic surface “beams” , . In highly nonlinear regime polaritons are predicted to display self-focusing effects and to form solitons .
Polariton–polariton interactions. The interaction of polaritons stems from their underlying matter constituents. In close analogy with other interacting systems, polariton–polariton interactions renormalize the dispersion and also prompt a blue shift of the emission energy as the polariton density increases , . Polariton–polariton interaction effects have been recently demonstrated for microcavity exciton polaritons , . See also quantum Hall polaritons.
Polaron polaritons. In TMDC monolayers, the itinerant electrons dynamically screen exciton to form new quasiparticle branches – the attractive and repulsive polaron – each with a renormalized mass and energy , . Microcavity polaritons with the matter constituent linked to these polaron branches are referred to as polaron polaritons .
Quantum Hall polaritons are a product of coupling cavity photons to the cyclotron resonance excitations of electron liquids in high-mobility semiconductor quantum wells or graphene sheets , . The edge channels of the quantum Hall effect offer a platform for probing interference and entanglement effects in the setting of a condensed matter system since the edge states propagation is ballistic, one-dimensional, and chiral. This platform enables experimental implementation of electron quantum optics , , ,  and may be suitable for the realization of flying qubits. In a parallel development, Smolka et al. . investigated cavity exciton polaritons in the presence of high-mobility 2D electron gas subjected to external magnetic field and discovered novel correlated electron phases. Knuppel et al.  reported on strong polariton–polariton interactions in the fractional quantum Hall regime.
Rydberg polaritons (QED): photons dressed by highly excited atomic Rydberg states under conditions of electromagnetic induced transparency. These polaritons can either reside in a cavity or propagate throughout an atomic ensemble. In a cavity, Rydberg dressing bestows an atomic ensemble with the character of a two-level system: the excitation of a single Rydberg polariton prevents the creation of a second one, in the so-called “Rydberg blockade” regime. Under conditions of electromagnetic induced transparency, polaritons can propagate within an optically dense atomic cloud. These polaritons can then be made to interact with each other via Rydberg dressing: the first Rydberg polariton alters the transparency condition for the second one, preventing its propagation within a certain “blockade radius” , , , . Rydberg polaritons are appealing for quantum logic functionalities  and for realizing synthetic materials via many-body states of light , .
Rydberg polaritons (QM): a special example of exciton polaritons with matter constituent associated with strongly interacting Rydberg states of excitons . Candidate systems include TMDC monolayers ,  and cuprous oxide, where Rydberg states with principal quantum numbers of up to n = 25 are feasible .
Soliton polaritons. Propagating wavepackets in semiconductor micorcavities are referred to as soliton polaritons (Figure 10C). In quantum optics, topological soliton polaritons refer to composite objects made of fermions trapped in an optical soliton. The prototypical one-dimensional (1D) model of solitons posessing nontrivial topology is the model of Su–Schrieffer–Heeger (SSH) chains . Variants of the SSH Hamiltonian have been emulated in the 1D lattices of microcavity exciton polaritons  and also in the system of quantum emitters coupled to a photonic waveguide . Topological phases of polritons in cavity waveguides were analyzed in a study by Downing et al. .
Spin polaritons: this term was coined in the context of polariton microcavity diode lasers operating via injection of spin polarized currents .
Spin plasmon polaritons are relevant to the plasmonic response of spin-polarized electron gas . Alternatively, spin–orbit interaction may lift the degeneracy between the spin states and give rise to transitions responsible for peculiar dispersion features of spin plasmon polaritons . The surface plasmon of a helical electron liquid is predicted to carry spin and is also referred to as a spin plasmon polariton .
Transformation optics with polaritons. Transformation optics refers to a general principle for designing a complex electromagnetic medium with tailored properties by carefully crafting the spatial patterns of the local optical index , . This general principle has been extended to polaritons  and polartonic cavities , and specifically to plasmon polaritons in graphene . Losses present the most significant experimental roadblock for practical transformational polaritonics. Recent advances with highly confined but low-loss plasmon polaritons  and phonon polaritons  fulfill important experimental preconditions for the realization of transformation optics ideas in polaritonic systems.
Tamm surface plasmon polaritons are associated with Tamm states at metallic surfaces . Common surface plasmon polaritons are formed with a TM polarization at the boundary of metallic and dielectric surfaces and lie to the right of the light cone. Tamm polaritons are found with both TM and transverse electric polarizations, and their dispersion can be within the light cone , .
Trion polaritons. The matter constituent of these polaritons is formed by charged excitons or trions (see also charged polaritons). Trion polaritons are commonly found in the response of TMDC semiconductors ,  and also in carbon nanotubes .
Tunneling plasmon polaritons were predicted  and observed  in an atomically thick tunable quantum tunneling devices consisting of two layers of graphene separated by 1 nm of h-BN. By applying a bias voltage between the graphene layers, one creates an electron gas coupled to a hole gas. Even though the total charge of the devices is zero, this system supports propagating graphene plasmons.
Valley polaritons. The matter constituent of these polaritons originates from valley polarized excitons in TMDC semiconductors (Figure 4B and exciton polaritons). The electronic structure of two-dimensional TMDC semiconductors endows this class of materials with the spin–valley degree of freedom that provides an optically accessible route for the control and manipulation of electron spin , , .
Vibrational polaritons: see molecular polaritons.
Wannier or Wannier–Mott polaritons borrow their matter part from Wannier excitons in semiconductors .
Waveguides and photonic crystals for polaritons. Waveguides and photonic crystals allow one to design and control the properties of photons, and thus of polaritons, both in quantum optics and QMs. In waveguide QED, different type of emitters (neutral atoms, quantum dots, color centers, superconducting qubits) are coupled to a one-dimensional (1D) optical channels , such as fibers , , photonic crystals , , and transmission lines ,  (Box 1 and Figure 11A). Channel with a bandgap give rise to atom–photon bound states (i.e., polaritonic bound states), provided the atomic resonance frequency is close to the band edge. Beyond the band-edge, photons are bound to the atoms, forming localized polaritonic cavities that can be harnessed for realizing quantum simulation and quantum information processing (Box 1). If the coupling between photons and atoms is strong enough, bound states emerge even if the atomic resonance frequency lies inside the band (i.e., as a “bound states in the continuum”) due to multiple scattering , . In the field of QMs, photonic crystal structures were fabricated using common phonon–polariton oxide systems LiTaO3 and LiNbO3 (Figure 11B). Pump–probe experiments in Figure 11B revealed the key attributes of the dispersion control by these periodic structures. A significant deficiency of conventional photonic crystals is that they do not allow for dynamical dispersion engineering. Xiong et al. circumvented this limitation and demonstrated a broadly tunable two-dimensional photonic crystal for surface plasmon polaritons [cross-ref-xiond]. Infrared nanoimaging revealed the formation of a photonic bandgap and an artificial domain wall which supports highly confined one-dimensional plasmonic modes.
Zenneck–Sommerfeld waves and Norton waves: an early example of a guided electromagnetic wave at the interface of media with negative and positive dielectric function , , , the same condition that is required for the formation of polaritonic modes in THz, infrared, and optical frequencies. The original prediction of Zenneck–Sommerfeld waves pertained to the radiofrequency wave at the interface of air and the Earth. In this analysis, the surface of the Earth was regarded as a lossy dielectric. The concept of Zenneck–Sommerfeld waves and closely related Norton waves has been applied to a broad class of wave patterns on the surface of metallic , , ,  and dielectric materials .
Funding source: U.S. Department of Energy (DOE)
Award Identifier / Grant number: DE-SC0019443
Funding source: Office of Science
Funding source: Basic Energy Sciences
Research at Columbia is supported as part of Programmable Quantum Materials, an Energy Frontier Research Center funded by the U.S. Department of Energy (DOE), Office of Science, Basic Energy Sciences (BES), under award DE-SC0019443. D.N.B. is Vannevar Bush Faculty Fellow ONR-VB: N00014-19-1-2630 and Moore Investigator in Quantum Materials #9455.
Author contribution: All the authors have accepted responsibility for the entire content of this submitted manuscript and approved submission.
Research funding: Research at Columbia is supported as part of Programmable Quantum Materials, an Energy Frontier Research Center funded by the U.S. Department of Energy (DOE), Office of Science, Basic Energy Sciences (BES), under award DE-SC0019443.
Conflict of interest statement: The authors declare no conflicts of interest regarding this article.
 D. N. Basov, M. M. Fogler, and F. J. Garcia de Abajo, “Polaritons in van der Waals materials,” Science, vol. 354, p. 195, 2016. https://doi.org/10.1126/science.aag1992.Search in Google Scholar PubMed
 D. N. Basov, R. D. Averitt and D. Hsieh, “Towards properties on demand in quantum materials,” Nat. Mater., vol. 16, p. 1077, 2017. https://doi.org/10.1038/nmat5017.Search in Google Scholar PubMed
 T. Low, A. Chaves, J. D. Caldwell, et al., “Polaritons in layered two-dimensional materials,” Nat. Mater., vol. 16, p. 182, 2017. https://doi.org/10.1038/nmat4792.Search in Google Scholar PubMed
 D. E. Chang, J. S. Douglas, A. Gonzalez-Tudela, C.-L. Hung, and H. J. Kimble, “Colloquium: Quantum matter built from a nanoscopic lattices of atoms and photons,” Rev. Mod. Phys., vol. 90, p. 031002, 2018. https://doi.org/10.1103/revmodphys.90.031002.Search in Google Scholar
 A. A. Clerk, K. W. Lehnert, P. Bertet, J. R. Petta and Y. Nakamura, “Hybrid quantum systems with circuit quantum electrodynamics,” Nat. Phys., vol. 16, p. 257, 2020. https://doi.org/10.1038/s41567-020-0797-9.Search in Google Scholar
 I. Carusotto, A. A. Houck, P. Roushan, D. I. Schuster, and J. Simon, “Photonic materials in circuit quantum electrodynamics,” Nat. Phys., vol. 16, p. 268, 2020. https://doi.org/10.1038/s41567-020-0815-y.Search in Google Scholar
 M. Ruggenthaler, N. Tancogne-Dejean, J. Flick, H. Appel, and A. Rubio, “From a quantum-electrodynamical light–matter description to novel spectroscopies,” Nat. Rev. Chem., vol. 2, p. 0118, 2018. https://doi.org/10.1038/s41570-018-0035-5.Search in Google Scholar
 P. Forn-Díaz, L. Lamata, E. Rico, J. Kono, and E. Solano, “Ultrastrong coupling regimes of light–matter interaction,” Rev. Mod. Phys., vol. 91, p. 025005, 2019. https://doi.org/10.1103/revmodphys.91.025005.Search in Google Scholar
 A. Michael, J. L. Sentef, F. Künzel, and M. Eckstein, “Quantum to classical crossover of Floquet engineering in correlated quantum system,s” Phys. Rev. Res., vol. 2, p. 033033, 2020.10.1103/PhysRevResearch.2.033033Search in Google Scholar
 A. F. Kockum, A. Miranowicz, S. De Liberato, S. Savasta, and F. Nori, “Ultrastrong coupling between light and matter,” Nat. Rev. Phys., vol. 1, p. 19, 2019. https://doi.org/10.1038/s42254-019-0046-2.Search in Google Scholar
 R. Jestädt, M. Ruggenthaler, M. J. T. Oliveira, A. Rubio, and H. Appel “Light–matter interactions within the Ehrenfest–Maxwell–Pauli–Kohn–Sham framework: fundamentals, implementation, and nano-optical applications,” Adv. Phys., vol. 68, p. 225, 2020. https://doi.org/10.1080/00018732.2019.1695875.Search in Google Scholar
 Z. M. Raines, A. A. Allocca, M. Hafezi, and V. M. Galitski, “Cavity Higgs polaritons,” Phys. Rev. Res., vol. 2, p. 013143, 2020. https://doi.org/10.1103/physrevresearch.2.013143.Search in Google Scholar
 Z. Sun, M. M. Fogler, D. N. Basov, and A. J. Millis, “Collective modes and THz near field response of superconductors,” Phys. Rev. Res., vol. 2, p. 023413, 2020. https://doi.org/10.1103/physrevresearch.2.023413.Search in Google Scholar
 P. B. Littlewood and C. M. Varma, “Gauge-invariant theory of the dynamical interaction of charge density waves and superconductivity” Phys. Rev. Lett., vol. 47, p. 811, 1981. https://doi.org/10.1103/physrevlett.47.811.Search in Google Scholar
 L. R. Walker, “Magnetostatic modes in ferromagnetic resonance,” Phys. Rev., vol. 105, p. 390, 1957. https://doi.org/10.1103/physrev.105.390.Search in Google Scholar
 A. A. Allocca, Z. M. Raines, J. B. Curtis, and V. M. Galitski, “Cavity superconductor-polaritons” Phys. Rev. B, vol. 99, p. 020504(R), 2019. https://doi.org/10.1103/physrevb.99.020504.Search in Google Scholar
 Z. Sun and A. Millis, “Bardasis–Schrieffer polaritons in excitonic insulators,” Phys. Rev. B, vol. 102, p. 041110, 2020. https://doi.org/10.1103/physrevb.102.041110.Search in Google Scholar
 H. T. Stinson, A. Sternbach, O. Najera, et al.., “Imaging the nanoscale phase separation in vanadium dioxide thin films at terahertz frequencies,” Nat. Commun., vol. 9, p. 3604, 2018. https://doi.org/10.1038/s41467-018-05998-5.Search in Google Scholar PubMed PubMed Central
 N. G. Basov, “Semiconductor lasers,” Science, vol. 149, p. 821, 1965. https://doi.org/10.1126/science.149.3686.821.Search in Google Scholar PubMed
 H. Deng, “Exciton-polariton Bose–Einstein condensation,” Rev. Mod. Phys., vol. 82, p. 1489, 2010. https://doi.org/10.1103/revmodphys.82.1489.Search in Google Scholar
 T. Schwartz, J. A. Hutchison, C. Genet, and T. W. Ebbesen, “Reversible switching of ultra-strong coupling,” Phys. Rev. Lett., vol. 106, p. 196405, 2011. https://doi.org/10.1103/physrevlett.106.196405.Search in Google Scholar
 S. Kéna-Cohen, S. A. Maier, and D. D. C. Bradley, “Ultrastrongly coupled exciton-polaritons in metal-clad organic semiconductor microcavities,” Adv. Opt. Mater., vol. 1, p. 827, 2013. https://doi.org/10.1002/adom.201300256.Search in Google Scholar
 L. Tian and H. J. Carmichael, “Quantum trajectory simulations of the two-state Behavior of an optical cavity containing one atom,” Phys. Rev. A, vol. 46, p. R6801, 1992. https://doi.org/10.1103/physreva.46.r6801.Search in Google Scholar PubMed
 A. Imamoğlu, H. Schmidt, G. Woods, and M. Deutsch, “Strongly interacting Photons in a nonlinear cavity,” Phys. Rev. Lett., vol. 79, p. 1467, 1997.10.1103/PhysRevLett.79.1467Search in Google Scholar
 J. S. Douglas, H. Habibian, C.-L. Hung, A. V. Gorshkov, H. J. Kimble and D. E. Chang, “Quantum many-body models with cold atoms coupled to photonic crystals,” Nat. Photonics, vol. 9, p. 326, 2015. https://doi.org/10.1038/nphoton.2015.57.Search in Google Scholar
 S. Dufferwiel, S. Schwarz, F. Withers, et al.., “Exciton-polaritons in van der waals heterostructures embedded in tunable microcavities,” Nat. Commun., vol. 6, p. 8579, 2015. https://doi.org/10.1038/ncomms9579.Search in Google Scholar PubMed PubMed Central
 N. Lundt, S. Klembt, E. Cherotchenko, et al.., “Room-temperature Tamm-plasmon exciton-polaritons with a WSe2 monolayer,” Nat. Commun., vol. 7, p. 13328, 2016. https://doi.org/10.1038/ncomms13328.Search in Google Scholar PubMed PubMed Central
 X. Liu, T. Galfsky, Z. Sun, et al.., “Strong light–matter coupling in two-dimensional atomic crystals,” Nat. Photonics, vol. 9, p. 30, 2015. https://doi.org/10.1038/nphoton.2014.304.Search in Google Scholar
 J. Sik, M. Schubert, T. Hofman and V. Gottschalch, Free-Carrier Effects and Optical Phonons in GaNAs/GaAs Superlattice Heterostructures Measured by Infrared Spectroscopic Ellipsometry, vol. 5, Cambridge University Press, 2014.10.1557/S109257830000003XSearch in Google Scholar
 E. L. Runnerstrom, K. P. Kelley, E. Sachet, C. T. Shelton, and J. P. Maria, “Epsilon-near-zero modes and surface plasmon resonance in fluorine-doped cadmium oxide thin films,” ACS Photonics, vol. 4, p. 188, 2017. https://doi.org/10.1021/acsphotonics.7b00429.Search in Google Scholar
 K. P. Kelley, E. L. Runnerstrom, E. Sachet, et al.., “Multiple epsilon-near-zero Resonances in multilayered cadmium oxide: designing metamaterial-like optical Properties in monolithic materials,” ACS Photonics, vol. 6, p. 1139, 2019. https://doi.org/10.1021/acsphotonics.9b00367.Search in Google Scholar
 A. Alù, M. G. Silveirinha, A. Salandrino, and N. Engheta, “Epsilon-near-zero metamaterials and electromagnetic sources: tailoring the radiation phase pattern,”Phys. Rev. B, vol. 75, p. 155410, 2007. https://doi.org/10.1103/physrevb.75.155410.Search in Google Scholar
 V. Bruno, C. DeVault, S. Vezzoli, et al.., “Negative refraction in time-varying strongly coupled plasmonic-antenna–epsilon-near-zero systems,” Phys. Rev. Lett., vol. 124, p. 043902, 2020. https://doi.org/10.1103/physrevlett.124.043902.Search in Google Scholar
 T. G. Folland, G. Lu, A. Bruncz, J. R. Nolen, M. Tadjer, and J. D. Caldwell, “Vibrational coupling to epsilon-near-zero waveguide modes,” ACS Photonics, vol. 7, p. 614, 2020. https://doi.org/10.1021/acsphotonics.0c00071.Search in Google Scholar
 M. H. Javani and M. I. Stockman, “Real and imaginary Properties of epsilon-near-zero materials,” Phys. Rev. Lett., vol. 117, p. 107404, 2016. https://doi.org/10.1103/physrevlett.117.107404.Search in Google Scholar PubMed
 D. Yoo, F. de Leon-Perez, I.-H. Lee, et al., “Ultrastrong plasmon-phonon coupling via epsilon-near-zero nanocavities,” arXiv:2003.00136, 2020.10.1038/s41566-020-00731-5Search in Google Scholar
 A. M. Mahmoud, Y. Li, B. Edwards, and N. Engheta, “Photonic doping of epsilon-near-zero media Iñigo Liberal,” Science, vol. 355, p. 10568, 2017.Search in Google Scholar
 J. C. W. Song and M. S. Rudner, “Chiral plasmons without magnetic field,” Proc. Natl. Acad. Sci. U.S.A., vol. 113, no. 17, p. 4658, 2016. https://doi.org/10.1073/pnas.1519086113.Search in Google Scholar PubMed PubMed Central
 A. Kumar, A. Nemilentsau, K. Hung Fung, G. Hanson, N. X. Fang, and T. Low, “Chiral plasmon in gapped Dirac systems,” Phys. Rev. B, vol. 93, p. 041413(R), 2016. https://doi.org/10.1103/physrevb.93.041413.Search in Google Scholar
 Li-kun Shi and Justin C. W. Song, “Plasmon geometric phase and plasmon Hall shift,” Phys. Rev. X, vol. 8, p. 021020, 2018. https://doi.org/10.1103/physrevx.8.021020.Search in Google Scholar
 P. M. J. Bhaseen, M. Hohenadler, A. O. Silver, and B. D. Simons, “Polaritons and pairing Phenomena in bose-hubbard mixtures,” Phys. Rev. Lett., vol. 102, p. 135301, 2009. https://doi.org/10.1103/physrevlett.102.135301.Search in Google Scholar
 P. Cilibrizzi, H. Sigurdsson, T. C. H. Liew, et al.., “Half-skyrmion spin textures in polariton microcavities,” Phys. Rev. B, vol. 94, p. 045315, 2016. https://doi.org/10.1103/physrevb.94.045315.Search in Google Scholar
 S. Donati, L. Dominici, G. Dagvadorj, et al.., “Twist of generalized skyrmions and spin vortices in a polariton superfluid,” Proc. Natl. Acad. Sci. U.S.A., vol. 113, p. 14926, 2016. https://doi.org/10.1073/pnas.1610123114.Search in Google Scholar
 H. Hubener, U. De Giovannini, C. Schafer, et al., “Quantum cavities and Floquet materials engineering: the power of chirality,” Nat. Mater. 2020 (in press).Search in Google Scholar
 V. D. Vaidya, Y. Guo, R. M. Kroeze, et al.., “Tunable-range, photon-mediated atomic interactions in multimode cavity QED,” Phys. Rev. X, vol. 8, p. 011002, 2018. https://doi.org/10.1103/physrevx.8.011002.Search in Google Scholar
 N. Jia, N. Schine, A. Georgakopoulos, et al.., “A strongly interacting polaritonic quantum dot,” Nat. Phys., vol. 14, p. 550, 2018. https://doi.org/10.1038/s41567-018-0071-6.Search in Google Scholar
 S. Faure, C. Brimont, T. Guillet, et al.., “Relaxation and emission of Bragg-mode and cavity-mode polaritons in a ZnO microcavity at room temperature,” Appl. Phys. Lett., vol. 95, p. 121102, 2009. https://doi.org/10.1063/1.3232228.Search in Google Scholar
 D. Goldberg, L. I. Deych, A. A. Lisyansky, et al.., “Exciton-lattice polaritons in multiple-quantum-well-based photonic crystals,” Nat. Photonics, vol. 3, p. 662, 2009. https://doi.org/10.1038/nphoton.2009.190.Search in Google Scholar
 E. S. Sedov, I. V. Iorsh, S. M. Arakelian, A. P. Alodjants, and A. Kavokin, “Hyperbolic metamaterials with Bragg polaritons,” Phys. Rev. Lett., vol. 114, p. 237402, 2015. https://doi.org/10.1103/physrevlett.114.237402.Search in Google Scholar
 C. Weisbuch and H. Benisty, “Microcavities in ecole polytechnique federale de lausanne, ecole polytechnique (France) and elsewhere: past, present and future,” Phys. Stat. Sol.(b), vol. 242, p. 2345, 2005. https://doi.org/10.1002/pssb.200560972.Search in Google Scholar
 A. Kavokin and G. Malpuech, Cavity Polaritons, vol. 32, p. 246, Academic Press, 2003.10.1016/S1079-4050(03)80003-0Search in Google Scholar
 P. G. Savvidis, J. J. Baumberg, R. M. Stevenson, M. S. Skolnick, D. M. Whittaker, and J. S. Roberts, “Angle-resonant stimulated polariton amplifier,” Phys. Rev. Lett., vol. 84, p. 1547, 2000. https://doi.org/10.1103/physrevlett.84.1547.Search in Google Scholar PubMed
 R. M. Stevenson, V. N. Astratov, M. S. Skolnick, et al.., “Continuous wave observation of massive polariton redistribution by stimulated scattering in semiconductor microcavities,” Phys. Rev. Lett., vol. 85, p. 3680, 2000. https://doi.org/10.1103/physrevlett.85.3680.Search in Google Scholar
 H. Deng, G. Weihs, C. Santori, J. Bloch, and Y. Yamamoto, “Condensation of semiconductor microcavity exciton polaritons” Science, vol. 298, p. 1999, 2002. https://doi.org/10.1126/science.1074464.Search in Google Scholar PubMed
 T. Guillet and C. Brimont, “Polariton condensates at room temperature,” Compt. Rendus Phys., vol. 17, p. 946, 2016. https://doi.org/10.1016/j.crhy.2016.07.002.Search in Google Scholar
 Á. Cuevas, J. C. López Carreño, B. Silva, et al.., “First observation of the quantized exciton-polariton field and effect of interactions on a single polariton,” Sci. Adv., vol. 4, p. eaao6814, 2018. https://doi.org/10.1126/sciadv.aao6814.Search in Google Scholar PubMed PubMed Central
 A. Delteil, T. Fink, A. Schade, S. Höfling, C. Schneider, and A. İmamoğlu, “Towards polariton blockade of confined exciton-polaritons,” Nat. Mater., vol. 18, p. 219, 2019. https://doi.org/10.1038/s41563-019-0282-y.Search in Google Scholar PubMed
 G. Muñoz-Matutano, A. Wood, M. Johnsson, et al.., “Emergence of quantum correlations from interacting fibre-cavity polaritons,” Nat. Mater., vol. 18, p. 213, 2019. https://doi.org/10.1038/s41563-019-0281-z.Search in Google Scholar PubMed
 S. S. Demirchyan, Y. Chestnov, A. P. Alodjants, M. M. Glazov, and A. V. Kavokin, “Qubits Based on polariton Rabi oscillators,” Phys. Rev. Lett., vol. 112, p. 196403, 2014. https://doi.org/10.1103/physrevlett.112.196403.Search in Google Scholar
 I. V. Novikov and A. A. Maradudin, “Channel polaritons” Phys. Rev. B, vol. 66, p. 035403, 2002. https://doi.org/10.1103/physrevb.66.035403.Search in Google Scholar
 S. I. Bozhevolnyi, V. S. Volkov, E. Devaux, J-, Y. Laluet, and T. W. Ebbesen, “Channel plasmon subwavelength waveguide components including interferometers and ring resonators,” Nature, vol. 440, p. 508, 2006. https://doi.org/10.1038/nature04594.Search in Google Scholar PubMed
 P. A. D. Gonca̧lves, S. Xiao, N. M. R. Peres, and N. Asger Mortensen, “Hybridized plasmons in 2D nanoslits: from Graphene to anisotropic 2D materials,” ACS Photonics, vol. 4, p. 3045, 2017.10.1021/acsphotonics.7b00558Search in Google Scholar
 Z. Fei, A. S. Rodin, G. O. Andreev, et al.., “Gate-tuning of graphene plasmons revealed by infrared nano-imaging,” Nature, vol. 487, p. 82, 2012. https://doi.org/10.1038/nature11253.Search in Google Scholar PubMed
 J. Chen, M. Badioli, P. Alonso-Gonzalez, et al., “Optical nano-imaging of gate-tunable graphene plasmons,” Nature, vol. 487, p. 77, 2012. https://doi.org/10.1038/nature11254.Search in Google Scholar PubMed
 M. D. Goldflam, G.-X. Ni, K. W. Post, et al., “Tuning and persistent switching of graphene plasmons on a ferroelectric substrate,” Nano Lett., vol. 15, p. 4859, 2015. https://doi.org/10.1021/acs.nanolett.5b00125.Search in Google Scholar PubMed
 S. Xiao, X. Zhu, B.-H. Li, and N. Asger Mortensen, “Graphene-plasmon polaritons: from fundamental properties to potential applications,” Front. Phys., vol. 11, p. 117801, 2016. https://doi.org/10.1007/s11467-016-0551-z.Search in Google Scholar
 M. Wagner, Z. Fei, A. S. McLeod, et al.., “Ultrafast and nanoscale plasmonic phenomena in exfoliated graphene revealed by infrared pump–probe nanoscopy,” Nano Lett., vol. 14, p. 894, 2014. https://doi.org/10.1021/nl4042577.Search in Google Scholar PubMed
 D. J. Rizzo, B. S. Jessen, Z. Sun, et al., “Graphene/α-RuCl3: an emergent 2D plasmonic interface,” arXiv:2007.07147, 2020.Search in Google Scholar
 F. Wen, Y. Zhang, S. Gottheim, et al.., “Charge transfer plasmons: optical frequency Conductances and tunable infrared resonances,” ACS Nano, vol. 9, p. 6428, 2015. https://doi.org/10.1021/acsnano.5b02087.Search in Google Scholar PubMed
 M. Forg, L. Colombier, R. K. Patel, et al.., “Cavity-control of interlayer excitons in van der Waals heterostructures,” Nat. Commun., vol. 10, p. 3697, 2019. https://doi.org/10.1038/s41467-019-11620-z.Search in Google Scholar PubMed PubMed Central
 R. Rapaport, R. Harel, E. Cohen, A. Ron, E. Linder, and L. N. Pfeiffer, “Negatively charged quantum well Polaritons in a GaAs/AlAs microcavity: an analog of atoms in a cavity,” Phys. Rev. Lett., vol. 84, p. 1607, 2000. https://doi.org/10.1103/physrevlett.84.1607.Search in Google Scholar PubMed
 J. M. Raimond and S. Haroche, “Confined electrons and photons,” edited by E. Burstein and C. Weisbuch, Springer- New Physics and Applications, vol. 383, 1995.10.1007/978-1-4615-1963-8_14Search in Google Scholar
 A. Tiene, J. Levinsen, M. M. Parish, A. H. MacDonald, J. Keeling, and F. M. Marchetti, “Extremely imbalanced two-dimensional electron–hole–photon systems,” Phys. Rev. Res., vol. 2, p. 023089, 2020. https://doi.org/10.1103/physrevresearch.2.023089.Search in Google Scholar
 P. A. Cherenkov. "Visible emission of clean liquids by action of γ radiation,” Dokl. Akad. Nauk SSSR, vol. 2, p. 451, 1934.Search in Google Scholar
 P. Genevet, D. Wintz, A. Ambrosio, A. She, R. Blanchard and F. Capasso, “Controlled steering of Cherenkov surface plasmon wakes with a one-dimensional metamaterial,” Nat. Nanotechnol., vol. 10, p. 804, 2015. https://doi.org/10.1038/nnano.2015.137.Search in Google Scholar PubMed
 D. H. Auston, K. P. Cheung, J. A. Valdmanis, and D. A. Kleinman, “Cherenkov radiation from femtosecond optical pulses in electro-optic media,” Phys. Rev. Lett., vol. 53, p. 1555, 1984. https://doi.org/10.1103/physrevlett.53.1555.Search in Google Scholar
 C. Maciel-Escudero, A. Koněcńa, R. Hillenbrand, and J. Aizpurua, “Probing and steering bulk and surface phonon polaritons in uniaxial materials using fast electrons: hexagonal boron nitride,” arXiv:2006.05359v1, 2020.10.1103/PhysRevB.102.115431Search in Google Scholar
 Y. Zhang, C. Hu, B. Lyu, et al.., “Tunable Cherenkov radiation of phonon Polaritons in silver nanowire/hexagonal boron nitride heterostructures,” Nano Lett., vol. 20, p. 2770, 2020. https://doi.org/10.1021/acs.nanolett.0c00419.Search in Google Scholar PubMed
 H. T. Stinson, J. S. Wu, B. Y. Jiang, et al.., “Infrared nanospectroscopy and imaging of collective superfluid excitations in anisotropic superconductors,” Phys. Rev. B, vol. 90, p. 014502, 2014. https://doi.org/10.1103/physrevb.90.014502.Search in Google Scholar
 A. Dodel, A. Pikovski, I. Ermakov, et al.., “Cooper pair polaritons in cold fermionic atoms within a cavity,” Phys. Rev. Res., vol. 2, p. 013184, 2020. https://doi.org/10.1103/physrevresearch.2.013184.Search in Google Scholar
 W. L. Barnes, A. Dereux, D T. W. Ebbesen, “Surface plasmon subwavelength optics,” Nature, vol. 424, p. 824, 2003. https://doi.org/10.1038/nature01937.Search in Google Scholar PubMed
 P. J. Schuck, D. P. Fromm, A. Sundaramurthy, G. S. Kino, and W. E. Moerner, “Improving the mismatch between light and nanoscale objects with gold bowtie nanoantennas,” Phys. Rev. Lett., vol. 94, p. 017402, 2005. https://doi.org/10.1103/physrevlett.94.017402.Search in Google Scholar
 P. Biagioni, J. S. Huang, and B. Hecht, “Nanoantennas for visible and infrared radiation,” Rep. Prog. Phys., vol. 75, p. 024402, 2012. https://doi.org/10.1088/0034-4885/75/2/024402.Search in Google Scholar PubMed
 L. Novotny and N. Van Hulst, “Antennas for light,” Nat. Photonics, vol. 5, p. 83, 2011. https://doi.org/10.1038/nphoton.2010.237.Search in Google Scholar
 J. J. Baumberg, J. Aizpurua, M. H. Mikkelsen, and D. R. Smith, “Extreme nanophotonics from ultrathin metallic gaps,” Nat. Mater., vol. 18, p. 668, 2019. https://doi.org/10.1038/s41563-019-0290-y.Search in Google Scholar PubMed
 M. Tamagnone, A. Ambrosio, K. Chaudhary, et al.., “Ultra-confined mid-infrared resonant phonon polaritons in van der Waals nanostructures,” Sci. Adv., vol. 4, p. eaat7189, 2018. https://doi.org/10.1126/sciadv.aat7189.Search in Google Scholar PubMed PubMed Central
 A. M. Dubrovkin, B. Qiang, T. Salim, D. Nam, N. I. Zheludey and Q. J. Wang, “Resonant nanostructures for highly confined and ultra-sensitive surface phonon-laritons,” Nat. Commun., vol. 11, p. 1863, 2020. https://doi.org/10.1038/s41467-020-15767-y.Search in Google Scholar PubMed PubMed Central
 L. V. Brown, M. Davanco, Z. Sun, et al.., “Nanoscale mapping and spectroscopy of nonradiative hyperbolic modes in hexagonal boron nitride nanostructures,” Nano Lett., vol. 18, p. 1628, 2018. https://doi.org/10.1021/acs.nanolett.7b04476.Search in Google Scholar PubMed PubMed Central
 X. Chen, D. Hu, R. Mescall, et al., “Modern scattering-type scanning near-field optical microscope for advanced material research,” Adv. Mater., vol. 31, p. 1804774, 2019. https://doi.org/10.1002/adma.201804774.Search in Google Scholar PubMed
 Z. Fei, G. O. Andreev, W. Bao, et al.., “Infrared nanoscopy of Dirac plasmons at the graphene–SiO2 interface,” Nano Lett., vol. 11, p. 4701, 2011. https://doi.org/10.1021/nl202362d.Search in Google Scholar PubMed
 P. J. Schuck, A. Weber-Bargioni, P. D. Ashby, D. F. Ogletree, A. Schwartzberg, and S. Cabrini, “Life beyond diffraction: opening new routes to materials characterization with next-generation optical near-field approaches,” Adv. Funct. Mater., vol. 23, p. 2539, 2013. https://doi.org/10.1002/adfm.201203432.Search in Google Scholar
 S. Berweger, J. M. Atkin, R. L. Olmon, and M. B. Raschke, “Light on the tip of a needle: plasmonic nanofocusing for spectroscopy on the nanoscale,” J. Phys. Chem. Lett., vol. 3, p. 945, 2012. https://doi.org/10.1021/jz2016268.Search in Google Scholar PubMed
 K. D. Park, T. Jiang, G. Clark, X. Xu, M. B. Raschke, “Radiative control of dark excitons at room temperature by nano-optical antenna-tip Purcell effect,” Nat. Nanotechnol., vol. 13, p. 59, 2017. https://doi.org/10.1038/s41565-017-0003-0.Search in Google Scholar PubMed
 B.-Y. Jiang, L. M. Zhang, A. H. Castro Neto, D. N. Basov, and M. M. Fogler, “Generalized spectral method for near-field optical microscopy,” J. Appl. Phys., vol. 119, p. 054305, 2016. https://doi.org/10.1063/1.4941343.Search in Google Scholar
 F. Keilmann and R. Hillenbrand, “Near-field microscopy by elastic light scattering from a tip,” J. Philos. Trans. R. Soc. Lond. Ser. A Math. Phys. Eng. Sci., vol. 362, p. 787, 2014.10.1098/rsta.2003.1347Search in Google Scholar PubMed
 J. M. Atkin, S. Berweger, A. C. Jones and M. B. Raschke, “Nano-optical imaging and spectroscopy of order, phases, and domains in complex solids,” Adv. Phys., vol. 61, p. 745, 2012. https://doi.org/10.1080/00018732.2012.737982.Search in Google Scholar
 M. Fleischhauer and M. D. Lukin, “Dark-state polaritons in electromagnetically induced transparency,” Phys. Rev. Lett., vol. 84, p. 5094, 2000. https://doi.org/10.1103/physrevlett.84.5094.Search in Google Scholar PubMed
 S. E. Harris, J. E. Field, and A. Imamoglu, “Nonlinear optical processes using electromagnetically induced transparency,” Phys. Rev. Lett., vol. 64, p. 1107, 1990. https://doi.org/10.1103/physrevlett.64.1107.Search in Google Scholar PubMed
 M. D. Lukin, “Colloquium: trapping and manipulating photon states in atomic ensembles,” Rev. Mod. Phys., vol. 75, p. 457, 2003. https://doi.org/10.1103/revmodphys.75.457.Search in Google Scholar
 M. Fleischhauer, A. Imamoglu and J. P. Marangos, “Electromagnetically induced transparency: optics in coherent media,” Rev. Mod. Phys., vol. 77, p. 633, 2005. https://doi.org/10.1103/revmodphys.77.633.Search in Google Scholar
 H. Zoubi and H. Ritsch, “Lifetime and emission characteristics of collective electronic excitations in two-dimensional optical lattices,” Phys. Rev. A, vol. 83, p. 063831, 2011. https://doi.org/10.1103/physreva.83.063831.Search in Google Scholar
 R. J. Bettles, S. A. Gardiner, and C. S. Adams, “Cooperative eigenmodes and scattering in one-dimensional atomic arrays,” Phys. Rev. A, vol. 94, p. 043844, 2016. https://doi.org/10.1103/physreva.94.043844.Search in Google Scholar
 A. Asenjo-Garcia, M. Moreno-Cardoner, A. Albrecht, H. J. Kimble, and D. E. Chang, “Exponential improvement in photon storage fidelities using subradiance and “selective radiance,” in atomic arrays” Phys. Rev. X, vol. 7, p. 031024, 2017. https://doi.org/10.1103/physrevx.7.031024.Search in Google Scholar
 E. Shahmoon, D. S. Wild, M. D. Lukin, and S. F. Yelin, “Cooperative resonances in light scattering from two-dimensional atomic arrays,” Phys. Rev. Lett., vol. 118, p. 113601, 2017. https://doi.org/10.1103/physrevlett.118.113601.Search in Google Scholar PubMed
 D. Pines, “Electron Interaction in solids,” Can. J. Phys., vol. 34, p. 1379, 1956. https://doi.org/10.1139/p56-154.Search in Google Scholar
 Z. Sun, D. N. Basov, and M. M. Fogler, “Universal linear and nonlinear electrodynamics of a Dirac fluid,” Proc. Natl. Acad. Sci. U.S.A., vol. 115, p. 3285, 2018. https://doi.org/10.1073/pnas.1717010115.Search in Google Scholar PubMed PubMed Central
 Z. Sun, D. N. Basov, and M. M. Fogler, “Adiabatic amplification of plasmons and demons in 2D systems,” Phys. Rev. Lett., vol. 117, p. 076805, 2016. https://doi.org/10.1103/physrevlett.117.076805.Search in Google Scholar
 M. Jablan, H. Buljan, and M. Soljačić, “Plasmonics in graphene at infrared frequencies,” Phys. Rev. B, vol. 80, p. 245435, 2009. https://doi.org/10.1103/physrevb.80.245435.Search in Google Scholar
 A. Woessner, M. B. Lundeberg, Y. Gao, et al.., “Highly confined low-loss plasmons in graphene-boron nitride heterostructures,” Nat. Mater., vol. 14, p. 421, 2015. https://doi.org/10.1038/nmat4169.Search in Google Scholar PubMed
 G. X. Ni, A. S. McLeod, Z. Sun, et al., “Fundamental limits to graphene plasmonics,” Nature, vol. 557, p. 530, 2018. https://doi.org/10.1038/s41586-018-0136-9.Search in Google Scholar PubMed
 M. I. Dyakonov, “New type of electromagnetic wave propagating at an interface,” Sov. Phys. JETP, vol. 67, p. 714, 1988.Search in Google Scholar
 O. Takayama, L. Crasovan, D. Artigas, and L. Torner, “Observation of Dyakonov surface waves,” Phys. Rev. Lett., vol. 102, p. 043903, 2009. https://doi.org/10.1103/physrevlett.102.043903.Search in Google Scholar
 J. Zubin and E. E. Narimanov, “Optical hyperspace for plasmons: Dyakonov states in metamaterials,” Appl. Phys. Lett., vol. 93, p. 221109, 2008.10.1063/1.3037208Search in Google Scholar
 S. Dai, M. Tymchenko, Y. Yang, et al.., “Manipulation and steering of hyperbolic surface polaritons in hexagonal boron nitride,” Adv. Mater., vol. 30, p. 1706358, 2018. https://doi.org/10.1002/adma.201706358.Search in Google Scholar PubMed
 F. J. Alfaro-Mozaz, P. Alonso-Gonzalez, S. Velez, et al., “Nanoimaging of resonating hyperbolic polaritons in linear boron nitride antennas,” Nat. Commun., vol. 8, p. 15624, 2017. https://doi.org/10.1038/ncomms15624.Search in Google Scholar PubMed PubMed Central
 I. Dolado, F. J. Alfaro-Mozaz, P. Li, et al.., “Nanoscale guiding of infrared light with hyperbolic volume and surface polaritons in van der Waals material ribbons,” Adv. Mater., vol. 32, p. 1906530, 2020. https://doi.org/10.1002/adma.201906530.Search in Google Scholar PubMed
 D. B. Mast, A. J. Dahm, and A. L. Fetter, “Observation of bulk and edge magnetoylasmons in a two-dimensional electron fluid,” Phys. Rev. Lett., vol. 54, p. 1706, 1985. https://doi.org/10.1103/physrevlett.54.1706.Search in Google Scholar
 V. A. Volkov and S. A. Mikhailov, “Edge magnetoplasmons: low frequency weakly damped excitations in inhomogeneous two-dimensional electron systems,” Radio Eng. Electron. Inst. USSR Acad. Sci. Zh. Eksp. Teor. Fiz., vol. 94, p. 217, 1988.Search in Google Scholar
 N. Kumada, P. Roulleau, B. Roche, et al.., “Resonant edge magnetoplasmons and their decay in graphene,” Phys. Rev. Lett., vol. 113, p. 266601, 2014. https://doi.org/10.1103/physrevlett.113.266601.Search in Google Scholar
 I. Petkovic, F. I. B. Williams and D. Christian Glattli, “Edge magnetoplasmons in graphene,” J. Phys. D Appl. Phys., vol. 47, 2014.10.1088/0022-3727/47/9/094010Search in Google Scholar
 M. L. Sadowski, G. Martinez, M. Potemski, C. Berger, and W. A. de Heer, “Landau level spectroscopy of ultrathin graphite layers,” Phys. Rev. Lett., vol. 97, p. 266405, 2006. https://doi.org/10.1103/physrevlett.97.266405.Search in Google Scholar PubMed
 Z. Jiang, E. A. Henriksen, L. C. Tung, et al.., “Infrared spectroscopy of Landau levels in graphene,” Phys. Rev. Lett., vol. 98, p. 197403, 2007. https://doi.org/10.1103/physrevlett.98.197403.Search in Google Scholar PubMed
 M. Orlita, C. Faugeras, R. Grill, et al.., “Carrier scattering from dynamical magneto-conductivity in quasineutral epitaxial graphene,” Phys. Rev. Lett., vol. 107, p. 216603, 2011. https://doi.org/10.1103/physrevlett.107.216603.Search in Google Scholar
 Z. G. Chen, Z. Shi, W. Yang, et al.., “Observation of an intrinsic bandgap and Landau level renormalization in graphene/boron-nitride heterostructures,” Nat. Commun., vol. 5, p. 4461, 2014. https://doi.org/10.1038/ncomms5461.Search in Google Scholar PubMed
 I. O. Nedoliuk, S. Hu, A. K. Geim, and A. B. Kuzmenko, “Colossal infrared and terahertz magneto-optical activity in a two-dimensional Dirac material,”Nat. Nano, vol. 14, p. 756, 2019. https://doi.org/10.1038/s41565-019-0489-8.Search in Google Scholar PubMed
 Z. Fei, M. D. Goldflam, J.-S. Wu, et al.., “Edge and surface plasmons in graphene nanoribbons,” Nano Lett., vol. 15, pp. 8271–8276, 2015. https://doi.org/10.1021/acs.nanolett.5b03834.Search in Google Scholar PubMed
 P. Li, I. Dolado, F. J. Alfaro-Mozaz, et al.., “Optical nanoimaging of hyperbolic surface polaritons at the Edges of van der Waals materials,” Nano Lett., vol. 17, p. 228, 2017. https://doi.org/10.1021/acs.nanolett.6b03920.Search in Google Scholar PubMed
 A. Y. Nikitin, P. Alonso-González, S. Vélez, et al.., “Real-space mapping of tailored sheet and edge plasmons in graphene nanoresonators,” Nat. Photonics, vol. 10, p. 239, 2016. https://doi.org/10.1038/nphoton.2016.44.Search in Google Scholar
 P. Berini, “Plasmon-polariton waves guided by thin lossy metal films of finite width: Bound modes of symmetric structures,” Phys. Rev. B, vol. 61, p. 10484, 2000. https://doi.org/10.1103/physrevb.61.10484.Search in Google Scholar
 M. Lorente-Crespo, G. C. Ballesteros, C. Mateo-Segura, and C. García-Meca, “Edge-plasmon whispering-gallery modes in nanoholes” Phys. Rev. Appl., vol. 13, p. 024050, 2020. https://doi.org/10.1103/physrevapplied.13.024050.Search in Google Scholar
 T. Rindzevicius, Y. Alaverdyan, B. Sepulveda, et al.., “Nanohole plasmons in optically thin gold films,” J. Phys. Chem. C, vol. 111, p. 1207, 2007. https://doi.org/10.1021/jp065942q.Search in Google Scholar
 A. Degiron, H. Lezec, N. Yamamoto, and T. Ebbe-sen, “Optical transmission properties of a single subwave-length aperture in a real metal,” Opt. Commun., vol. 239, p. 61, 2004. https://doi.org/10.1016/j.optcom.2004.05.058.Search in Google Scholar
 N. Liu, L. Langguth, T. Weiss, et al.., “Plasmonic analogue of electromagnetically induced transparency at the Drude damping limit,” Nat. Mater., vol. 8, p. 758, 2009. https://doi.org/10.1038/nmat2495.Search in Google Scholar PubMed
 R. Taubert, M. Hentschel, J. Kastel, and H. Gissen, “Classical analog of electromagnetically induced absorption in plasmonics,” Nano Lett., vol. 12, p. 1367, 2012. https://doi.org/10.1021/nl2039748.Search in Google Scholar PubMed
 H. Yan, T. Low, F. Guinea, F. Xia, and P. Avouris, “Tunable phonon-induced transparency in bilayer graphene nanoribbons,” Nano Lett., vol. 14, p. 4581, 2014. https://doi.org/10.1021/nl501628x.Search in Google Scholar PubMed
 S. Xia, X. Zhai, L. Wang, and S. Wen, “Plasmonically induced transparency in in-plane isotropic and anisotropic 2D materials,” Opt. Express, vol. 28, p. 7980, 2020. https://doi.org/10.1364/oe.389573.Search in Google Scholar
 V. Walther, R. Johne and T. Pohl, “Giant optical nonlinearities from Rydberg excitons in semiconductor microcavities,” Nat. Commun., vol. 9, p. 1309, 2018. https://doi.org/10.1038/s41467-018-03742-7.Search in Google Scholar PubMed PubMed Central
 C. Weisbuch, M. Nishioka, A. Ishikawa, and Y. Arakawa, “Observation of the coupled exciton-photon mode splitting in a semiconductor quantum microcavity,” Phys. Rev. Lett., vol. 69, p. 3314, 1992. https://doi.org/10.1103/physrevlett.69.3314.Search in Google Scholar
 J. Kasprzak, M. Richard, S. Kundermann, et al.., “Bose–Einstein condensation of exciton polaritons” Nature, vol. 443, p. 409, 2006. https://doi.org/10.1038/nature05131.Search in Google Scholar PubMed
 I. Carusotto and C. Ciuti, “Quantum fluids of light,” Rev. Mod. Phys., vol. 85, p. 29,2013. https://doi.org/10.1103/revmodphys.85.299.Search in Google Scholar
 T. Byrnes, N. Y. Kim, and Y. Yamamoto, “Exciton-polariton condensates,” Nat. Phys., vol. 10, p. 803, 2014. https://doi.org/10.1038/nphys3143.Search in Google Scholar
 A. Griffin, D. W. Snoke, and S. Stringari, eds., Bose–Einstein Condensation, Cambridge University Press, 1996.10.1017/CBO9780511524240Search in Google Scholar
 A. A. High, J. R. Leonard, A. T. Hammack, et al.., “Spontaneous coherence in a cold exciton gas,” Nature, vol. 483, p. 7391, 2012. https://doi.org/10.1038/nature10903.Search in Google Scholar PubMed
 D. Snoke, “Spontaneous Bose coherence of excitons and polaritons,” Science, vol. 298, p. 1368, 2002. https://doi.org/10.1126/science.1078082.Search in Google Scholar PubMed
 J. P. Eisenstein and A. H. MacDonald, “Bose–Einstein condensation of excitons in bilayer electron systems,” Nature, vol. 432, p. 691, 2004. https://doi.org/10.1038/nature03081.Search in Google Scholar PubMed
 H. Deng, H. Haug, and Y. Yamamoto, “Exciton-polariton Bose-Einstein condensation,” Rev. Mod. Phys., vol. 82, p. 1489, 2010. https://doi.org/10.1103/revmodphys.82.1489.Search in Google Scholar
 D. W. Snoke and J. Keeling, “The new era of polariton condensates,” Phys. Today, vol. 70, p. 54, 2017. https://doi.org/10.1063/pt.3.3729.Search in Google Scholar
 Y. Sun, P. Wen, Y. Yoon, et al.., “Bose–Einstein condensation of long-lifetime polaritons in thermal equilibrium,” Phys. Rev. Lett., vol. 118, p. 016602, 2017. https://doi.org/10.1103/physrevlett.118.149901.Search in Google Scholar PubMed
 G. Lerario, A. Fieramosca, F. Barachati, et al., “Room-temperature superfluidity in a polariton condensate,” Nat. Phys., vol. 13, p. 837, 2013.10.1038/nphys4147Search in Google Scholar
 Y. Fu, H. Zhu, J. Chen, M. P. Hautzinger, X.-Y. Zhu, and S. Jin, “Metal halide perovskite nanostructures for optoelectronic applications and the study of physical properties,” Nat. Rev. Mater., vol. 4, p. 169, 2019. https://doi.org/10.1038/s41578-019-0080-9.Search in Google Scholar
 A. T. Hanbicki, M. Currie, G. Kioseoglou, A. L. Friedman, and B. T. Jonker, “Measurement of high exciton binding energy in the monolayer transition-metal dichalcogenides WS2 and WSe2,” Sol. State. Commun., vol. 203, p. 16, 2015. https://doi.org/10.1016/j.ssc.2014.11.005.Search in Google Scholar
 T. Cheiwchanchamnangij and W. R. L. Lambrecht, “Quasiparticle band structure calculation of monolayer, bilayer, and bulk MoS2,” Phys. Rev. B, vol. 85, p. 205302, 2012. https://doi.org/10.1103/physrevb.85.205302.Search in Google Scholar
 A. Ramasubramaniam, “Large excitonic effects in monolayers of molybdenum and tungsten dichalcogenides,” Phys. Rev. B, vol. 86, p. 115409, 2012. https://doi.org/10.1103/physrevb.86.115409.Search in Google Scholar
 H.-P. Komsa and A. V. Krasheninnikov, “Effects of confinement and environment on the electronic structure and exciton binding energy of MoS2 from first principles,” Phys. Rev. B, vol. 86, p. 241201, 2012. https://doi.org/10.1103/physrevb.86.241201.Search in Google Scholar
 Y. Liang, S. Huang, R. Soklaski, and L. Yang, “Quasiparticle band-edge energy and band offsets of monolayer of molybdenum and tungsten chalcogenides,” Appl. Phys. Lett., vol. 103, p. 042106, 2013. https://doi.org/10.1063/1.4816517.Search in Google Scholar
 K. He, N. Kumar, L. Zhao, et al.., “Tightly bound excitons in monolayer WSe2,” Phys. Rev. Lett., vol. 113, p. 026803, 2014. https://doi.org/10.1103/physrevlett.113.026803.Search in Google Scholar
 Z. Ye, T. Cao, K. O’Brien, et al.., “Probing excitonic dark states in single-layer tungsten disulphide,” Nature, vol. 513, p. 214, 2014. https://doi.org/10.1038/nature13734.Search in Google Scholar PubMed
 K. Yao, A. Yan, S. Kahn, et al.., “Optically discriminating carrier-induced quasiparticle band gap and exciton energy renormalization in monolayer MoS2,” Phys. Rev. Lett., vol. 119, p. 087401, 2017. https://doi.org/10.1103/physrevlett.119.087401.Search in Google Scholar
 H. Min, R. Bistritzer, J. Su and A. H. MacDonald, “Room-temperature superfluidity in graphene bilayers” Phys. Rev. B, vol. 78, p. 121401, 2008. https://doi.org/10.1103/physrevb.78.121401.Search in Google Scholar
 M. M. Fogler, L. V. Butov, and K. S. Novoselov, “High-temperature superfluidity with indirect excitons in van der Waals heterostructures” Nat. Commun., vol. 5, p. 4555, 2014. https://doi.org/10.1038/ncomms5555.Search in Google Scholar PubMed
 F.-C. Wu, F. Xue, and A. H. MacDonald, “Theory of two-dimensional spatially indirect equilibrium exciton condensates,” Phys. Rev. B, vol. 92, p. 165121, 2015. https://doi.org/10.1103/physrevb.92.239901.Search in Google Scholar
 A. V. Nalitov, H. Sigurdsson, S. Morina, et al.., “Optically trapped polariton condensates as semiclassical time crystals,” Phys. Rev. A, vol. 99, p. 033830, 2019. https://doi.org/10.1103/physreva.99.033830.Search in Google Scholar
 M. D. Fraser, S. Hofling, and Y. Yamamoto, “Physics and applications of exciton-polariton lasers,” Nat. Mater., vol. 15, p. 1049, 2016. https://doi.org/10.1038/nmat4762.Search in Google Scholar PubMed
 A. Gianfrate, L. Dominici, O. Voronych, et al.., “Superluminal X-waves in a polariton quantum fluid,” Light Sci. Appl., vol. 7, p. 17119, 2018. https://doi.org/10.1038/lsa.2017.119.Search in Google Scholar PubMed PubMed Central
 A. Gabbay, Y. Preezant, E. Cohen, B. M. Ashkinadze and L. N. Pfeffier, “Fermi edge Polaritons in a microcavity containing a high-density two-dimensional electron gas,”Phys. Rev. Lett., vol. 99, p. 157402, 2007. https://doi.org/10.1103/physrevlett.99.157402.Search in Google Scholar PubMed
 D. Pimenov, J. von Delft, L. Glazman, and M. Goldstein, “Fermi-edge exciton-polaritons in doped semiconductor microcavities with finite hole mass,” Phys. Rev. B, vol. 96, p. 155310, 2017. https://doi.org/10.1103/physrevb.96.155310.Search in Google Scholar
 M. Baetena and M. Wouters, “Mahan polaritons and their lifetime due to hole recoil,” Eur. Phys. J. D, vol. 69, p. 243, 2015. https://doi.org/10.1140/epjd/e2015-60401-4.Search in Google Scholar
 G. D. Mahan, “Excitons in degenerate semiconductors,” Phys. Rev., vol. 153, p. 882, 1967. https://doi.org/10.1103/physrev.153.882.Search in Google Scholar
 G. D. Mahan, “Excitons in metals” Phys. Rev. Lett., vol. 18, p. 448, 1967. https://doi.org/10.1103/physrevlett.18.448.Search in Google Scholar
 T. Oka and S. Kitamura, “Floquet engineering of quantum materials,” Ann. Rev. Condensed Matter Phys., vol. 10, p. 387, 2019. https://doi.org/10.1146/annurev-conmatphys-031218-013423.Search in Google Scholar
 L. W. Clark, N. Jia, N. Schine, C. Baum, A. Georgakopoulos, and J. Simon, “Interacting Floquet polaritons,” Nature, vol. 571, p. 532, 2019. https://doi.org/10.1038/s41586-019-1354-5.Search in Google Scholar PubMed
 F. Mahmood, C.-K. Chan, Z. Alpichshev, et al.., “Selective scattering between Floquet-Bloch and Volkov states in a topological insulator,” Nat. Phys., vol. 12, p. 306, 2016. https://doi.org/10.1038/nphys3609.Search in Google Scholar
 H. Hübener, U. D. Giovannini, and A. Rubio, “Phonon driven Floquet matter,” Nano Lett., vol. 18, p. 1535, 2018. https://doi.org/10.1021/acs.nanolett.7b05391.Search in Google Scholar PubMed
 J.-M. Ménard, C. Poellmann, M. Porer, et al., “Revealing the dark side of a bright exciton-polariton condensate,” Nat. Commun., vol. 5, p. 4648, 2018.10.1038/ncomms5648Search in Google Scholar PubMed PubMed Central
 Z. Sun, J. Gu, A. Ghazaryan, et al.., “Optical control of room-temperature valley polaritons,” Nat. Photonics, vol. 11, p. 491, 2017. https://doi.org/10.1038/nphoton.2017.121.Search in Google Scholar
 L. Vestergaard Hau, S. E. Harris, Z. Dutton, and C. H. Behroozi, “Light speed reduction to 17 metres per second in an ultracold atomic gas,” Nature, vol. 397, p. 594, 1999. https://doi.org/10.1038/17561.Search in Google Scholar
 O. Kocharovskaya, Y. Rostovtsev, and M. O. Scully, “Stopping light via hot atoms,” Phys. Rev. Lett., vol. 86, p. 628, 2001. https://doi.org/10.1103/physrevlett.86.628.Search in Google Scholar
 M. Bajcsy, A. S. Zibrov, and M. D. Lukin, “Stationary pulses of light in an atomic medium,” Nature, vol. 426, p. 638, 2003. https://doi.org/10.1038/nature02176.Search in Google Scholar PubMed
 S. Betzold, M. Dusel, O. Kyriienko, et al.., “Coherence and Interaction in confined room-temperature polariton condensates with Frenkel excitons,” ACS Photonics, vol. 7, p. 384, 2020. https://doi.org/10.1021/acsphotonics.9b01300.Search in Google Scholar
 D. G. Lidzey, D. D. C. Bradley, T. Virgili, S. Walker, and D. M. Walker, “Strong exciton–photon coupling in an organic semiconductor microcavity,” Nature, vol. 395, p. 53, 1998. https://doi.org/10.1038/25692.Search in Google Scholar
 G. Lerario, A. Fieramosca, F. Barachati, et al.., “Room-temperature superfluidity in a polariton condensate,” Nat. Phys., vol. 13, p. 837, 2017. https://doi.org/10.1038/nphys4147.Search in Google Scholar
 J. Keeling and S. Kena-Cohen, “Bose–Einstein condensation of exciton-polariton in organic microcavities,” Annu. Rev. Phys. Chem., vol. 71, p. 435, 2020. https://doi.org/10.1146/annurev-physchem-010920-102509.Search in Google Scholar PubMed
 S. Foteinopoulou, G. Chinna Rao Devarapu, G. S. Subramania, S. Krishna and D. Wasserman, “Phonon-polaritonics: enabling powerful capabilities for infrared photonics,” Nanophotonics, vol. 8, p. 2129, 2019. https://doi.org/10.1515/nanoph-2019-0232.Search in Google Scholar
 K. I. Kliewer and R. Fuchs, “Optical modes of vibration in an ionic crystal slab including retardation. I. Nonradiative region,” Phys. Rev., vol. 144, p. 495, 1966. https://doi.org/10.1103/physrev.144.495.Search in Google Scholar
 A. Huber, N. Ocelic, D. V. Kazantsev, and R. Hillenbrand, “Near-field imaging of mid-infrared surface phonon polariton propagation,” Appl. Phys. Lett., vol. 87, p. 081103, 2005. https://doi.org/10.1063/1.2032595.Search in Google Scholar
 R. Hillenbrand, T. Taubner and F. Keilmann, “Phonon-enhanced light-matter interaction at the nanometre scale,” Nature, vol. 418, p. 159, 2002. https://doi.org/10.1038/nature00899.Search in Google Scholar PubMed
 J. D. Caldwell, O. J. Glembocki, N. Sharac, et al.., “Low-loss, extreme sub-diffraction photon confinement via silicon carbide surface phonon polariton nanopillar resonators,” Nano Lett., vol. 13, p. 3690, 2013. https://doi.org/10.1021/nl401590g.Search in Google Scholar PubMed
 T. E. Tiwald, J. A. Woolam, S. Zollner, et al.., “Carrier concentration and lattice absorption in bulk and epitaxial silicon carbide determined using infrared ellipsometry,” Phys. Rev. B, vol. 60, p. 11464, 1999. https://doi.org/10.1103/physrevb.60.11464.Search in Google Scholar
 T. Taubner, D. Korobkin, Y. Urzhumov, G. Shvets, and R. Hillenbrand, “Near-field microscopy through a SiC superlens,” Science, vol. 313, p. 1595, 2006. https://doi.org/10.1126/science.1131025.Search in Google Scholar PubMed
 W. J. Moore and R. T. Holm. “Infrared dielectric constant of GaAs,” J. Appl. Phys., vol. 80, p. 6939, 1996. https://doi.org/10.1063/1.363818.Search in Google Scholar
 M. Francesco, D. Pellegrino, M. I. Katsnelson, and M. Polini, “Helicons in Weyl semimetals,” Phys. Rev. B, vol. 92, p. 201407, 2015.10.1103/PhysRevB.92.201407Search in Google Scholar
 J. Zhou, H.-R. Chang, and D. Xiao, “Plasmon mode as a detection of the chiral anomaly in Weyl semimetals,” Phys. Rev. B, vol. 91, p. 035114, 2015. https://doi.org/10.1103/physrevb.91.035114.Search in Google Scholar
 C. Justin W. Song, and M. S. Rudner, “Fermi arc plasmons in Weyl semimetals,” Phys. Rev. B, vol. 96, p. 205443, 2017.10.1103/PhysRevB.96.205443Search in Google Scholar
 I. Iorsh, G. Rahmanova, and M. Titov, “Plasmon-polariton from a helical state in a Dirac magnet,” ACS Photonics, vol. 6, p. 2450, 2019. https://doi.org/10.1021/acsphotonics.9b00683.Search in Google Scholar
 J. Lin, J. P. Bathasar Mueller, Q. Wang, et al.., “Polarization-controlled tunable directional coupling of surface plasmon polaritons,” Science, vol. 340, p. 331, 2013. https://doi.org/10.1126/science.1233746.Search in Google Scholar PubMed
 L. Huang, X. Chen, B. Bai, et al.., “Helicity dependent directional surface plasmon polariton excitation using a metasurface with interfacial phase discontinuity,” Light Sci. Appl., vol. 2, p. 70, 2013. https://doi.org/10.1038/lsa.2013.26.Search in Google Scholar
 J. J. Hopfield, “Theory of the contribution of excitons to the complex dielectric constant of crystals,” Phys. Rev., vol. 112, p. 1555, 1958. https://doi.org/10.1103/physrev.112.1555.Search in Google Scholar
 C. H. Henry and J. J. Hopfield, “Raman scattering by polaritons,” Phys. Rev. Lett., vol. 15, p. 964, 1965. https://doi.org/10.1103/physrevlett.15.964.Search in Google Scholar
 U. Fano, “Atomic theory of electromagnetic interactions in dense materials,” Phys. Rev., vol. 103, p. 1202, 1956. https://doi.org/10.1103/physrev.103.1202.Search in Google Scholar
 K. Huang, “Lattice vibrations and optical waves in ionic crystals,” Nature, vol. 167, p. 779, 1951. https://doi.org/10.1038/167779b0.Search in Google Scholar
 K. B. Tolpygo, “Physical properties of a rock salt lattice made up of deformeable ions,” Translated and reprinted from Zh. Eksp. Teor. Fiz., vol. 20, no. 6, p. 497, 1950.Search in Google Scholar
 J. D. Caldwell, I. Vurgaftman, J. G. Tischler, O. J. Glembocki, J. C. Owrutsky, and T. L. Reinecke, “Atomic-scale photonic hybrids for mid-infrared and terahertz nanophotonics,” Nat. Nanotechnol., vol. 11, p. 9, 2016. https://doi.org/10.1038/nnano.2015.305.Search in Google Scholar PubMed
 L. Wendler and R. Haupt, “Long-range surface plasmon-phonon-polaritons,” J. Phys. C Solid State Phys., vol. 19, p. 1871, 1986. https://doi.org/10.1088/0022-3719/19/11/023.Search in Google Scholar
 B. Askenazi, A. Vasanelli, A. Delteil, et al.., “Ultra-strong light–matter coupling for designer Reststrahlen band,” New J. Phys., vol. 16, p. 043029, 2014. https://doi.org/10.1088/1367-2630/16/4/043029.Search in Google Scholar
 C. Franckié, K. Ndebeka-Bandou, J. Ohtani, and M. Faist, “Quantum model of gain in phonon-polariton lasers,” Phys. Rev. B, vol. 97, p. 075402, 2018. https://doi.org/10.1103/physrevb.97.075402.Search in Google Scholar
 N. C. Passler, C. R. Gubbin, T. G. Folland, et al.., “Strong coupling of epsilon-near-zero phonon Polaritons in polar dielectric heterostructures,” Nano Lett., vol. 18, p. 428, 2018. https://doi.org/10.1021/acs.nanolett.8b01273.Search in Google Scholar PubMed
 A. A. Strashko and V. M. Agranovich, “To the theory of surface plasmon-polaritons on metals covered with resonant thin films,” Opt. Commun., vol. 332, p. 201, 2014. https://doi.org/10.1016/j.optcom.2014.06.069.Search in Google Scholar
 D. C. Ratchford, C. J. Winta, I. Chatzakis, et al.., “Controlling the infrared dielectric function through atomic-scale heterostructures,” ACS Nano, vol. 13, p. 6730, 2019. https://doi.org/10.1021/acsnano.9b01275.Search in Google Scholar PubMed PubMed Central
 E. L. Runnerstrom, K. P. Kelley, T. G. Folland, et al.., “Polaritonic hybrid-epsilon-near-zero modes: beating the plasmonic confinement vs propagation-length trade-off with doped cadmium oxide bilayers,” Nano Lett., vol. 19, p. 948, 2019. https://doi.org/10.1021/acs.nanolett.8b04182.Search in Google Scholar PubMed
 K. Chaudhary, M. Tamagnone, M. Resaee, et al.., “Engineering phonon polaritons in van der Waals heterostructures to enhance in-plane optical anisotropy,” Sci. Adv., vol. 5, p. eaau7171, 2019. https://doi.org/10.1126/sciadv.aau7171.Search in Google Scholar PubMed PubMed Central
 S. Dai, Q. Ma, M. K. Liu, et al.., “Graphene on hexagonal boron nitride as a tunable hyperbolic metamaterial,” Nat. Nanotechnol., vol. 10, p. 682, 2015. https://doi.org/10.1038/nnano.2015.131.Search in Google Scholar PubMed
 F. J. Bezares, A. De Sanctis, J. R. M. Saavedra, et al.., “Intrinsic plasmon-phonon interactions in highly doped graphene: a near-field imaging study,” Nano Lett., vol. 17, p. 5908, 2017. https://doi.org/10.1021/acs.nanolett.7b01603.Search in Google Scholar PubMed
 A. Kumar, T. Low, K. Hung Fung, P. Avouris, and N. X. Fang, “Tunable light–matter interaction and the role of hyperbolicity in graphene-hBN system,” Nano Lett., vol. 15, p. 3172, 2015. https://doi.org/10.1021/acs.nanolett.5b01191.Search in Google Scholar PubMed
 A. T. Costa, P. A. D. Gonçalves, H. Frank, et al., “Harnessing ultra-confined graphene plasmons to probe the electrodynamics of superconductors,” arXiv:2006.00748, 2020.Search in Google Scholar
 H. Dehghani, Z. M. Raines, V. M. Galitski, and M. Hafezi, “Optical enhancement of superconductivity via targeted destruction of charge density waves,” Phys. Rev. B, vol. 101. p. 195106, 2020. https://doi.org/10.1103/physrevb.101.224506.Search in Google Scholar
 D. Rodrigo, O. Limaj, D. Janner, et al.., “Mid-infrared plasmonic biosensing with graphene,” Science, vol. 349, p. 165, 2015. https://doi.org/10.1126/science.aab2051.Search in Google Scholar PubMed
 M. Autore, P. Li, I. Dolado, et al.., “Boron nitride nanoresonators for phonon-enhanced molecular vibrational spectroscopy at the strong coupling limit,” Light Sci. Appl., vol. 7, p. 17172, 2018. https://doi.org/10.1038/lsa.2017.172.Search in Google Scholar PubMed PubMed Central
 C. R. Gubbin, R. Berte, M. A. Meeker, et al.., “Hybrid longitudinal-transverse phonon polaritons,” Nat. Commun., vol. 10, p. 1682, 2019. https://doi.org/10.1038/s41467-019-09414-4.Search in Google Scholar PubMed PubMed Central
 T. G. Folland, A. Fali, S. T. White, et al.., “Reconfigurable infrared hyperbolic metasurfaces using phase change materials,” Nat. Commun., vol. 9, p. 4371, 2018. https://doi.org/10.1038/s41467-018-06858-y.Search in Google Scholar PubMed PubMed Central
 A. Poddubny, I. Iorsh, P. Belov, and Y. Kivshar, “Hyperbolic metamaterials,” Nat. Photonics, vol. 7, p. 948, 2013. https://doi.org/10.1038/nphoton.2013.243.Search in Google Scholar
 J. S. Gomez-Diaz and A. Alu, “Flatland optics with hyperbolic metasurfaces,” ACS Photonics, vol. 3, p. 2211, 2016. https://doi.org/10.1021/acsphotonics.6b00645.Search in Google Scholar
 J. S. Gomez-Diaz, M. Tymchenko, and A. Alù, “Hyperbolic plasmons and topological transitions over uniaxial metasurfaces,” Phys. Rev. Lett., vol. 114, p. 233901, 2015. https://doi.org/10.1103/physrevlett.114.233901.Search in Google Scholar PubMed
 J. D. Caldwell, A. V. Kretinin, Y. Chen, et al.., “Sub-diffractional volume-confined polaritons in the natural hyperbolic material hexagonal boron nitride,” Nat. Commun., vol. 5, p. 5221, 2014. https://doi.org/10.1038/ncomms6221.Search in Google Scholar PubMed
 Y. Guo, W. Newman, C. L. Cortes, and Z. Jacob, “Applications of hyperbolic metamaterial substrates,” Adv. Optoelectron. 452502, (2012).10.1155/2012/452502Search in Google Scholar
 C. L. Cortes, W. Newman, S. Molesky and Z. Jacob “Quantum nanophotonics using hyperbolic metamaterials,” J. Opt., vol. 14, p. 063001, 2012. https://doi.org/10.1088/2040-8978/14/6/063001.Search in Google Scholar
 J. Sun, N. M. Litchinitser, and J. Zhou, “Indefinite by nature: from ultraviolet to terahertz,” ACS Photonics, vol. 1, p. 293, 2014. https://doi.org/10.1021/ph4000983.Search in Google Scholar
 E. E. Narimanov and A. V. Kildishev, “Metamaterials naturally hyperbolic,” Nat. Photonics, vol. 9, p. 214, 2015. https://doi.org/10.1038/nphoton.2015.56.Search in Google Scholar
 S. Dai, Z. Fei, Q. Ma, et al.., “Tunable phonon polaritons in atomically thin van der Waals crystals of boron nitride,” Science, vol. 343, p. 1125, 2014. https://doi.org/10.1126/science.1246833.Search in Google Scholar PubMed
 A. J. Giles, S. Dai, I. Vurgaftman, et al.., “Ultralow-loss polaritons in isotopically pure boron nitride,” Nat. Mater., vol. 17, p. 134, 2017. https://doi.org/10.1038/nmat5047.Search in Google Scholar PubMed
 J. Taboada-Gutiérrez, G. Álvarez-Pérez, J. Duan, et al.., “Broad spectral tuning of ultra-low-loss polaritons in a van der Waals crystal by intercalation,” Nat. Mater., vol. 19, p. 964, 2020. https://doi.org/10.1038/s41563-020-0665-0.Search in Google Scholar PubMed
 J. D. Caldwell, I. Aharonovich, G. Cassabois, J. H. Edgar, B. Gil and D. N. Basov, “Photonics with hexagonal boron nitride” Nat. Mater. Rev., vol. 4, no. 8, p. 552, 2019. https://doi.org/10.1038/s41578-019-0124-1.Search in Google Scholar
 A. Fali, S. T. White, T. G. Folland, et al.., “Refractive index-based Control of hyperbolic phonon-polariton propagation,” Nano Lett., vol. 9, no. 11, 7725–7730, 2019. https://doi.org/10.1021/acs.nanolett.9b02651.Search in Google Scholar PubMed
 A. Ambrosio, L. A. Jauregui, S. Dai, et al.., “Mechanical detection and imaging of hyperbolic phonon polaritons in hexagonal boron nitride,” ACS Nano, vol. 11, p. 8741, 2017. https://doi.org/10.1021/acsnano.7b02323.Search in Google Scholar PubMed
 A. Ambrosio, M. Tamagnone, K. Chaudhary, et al.., “Selective excitation and imaging of ultraslow phonon polaritons in thin hexagonal boron nitride crystals,” Light Sci. Appl., vol. 7, p. 27, 2018. https://doi.org/10.1038/s41377-018-0039-4.Search in Google Scholar PubMed PubMed Central
 G. Hu, J. Shen, C. W. Qiu, A. Alù, and S. Dai, “Phonon Polaritons and hyperbolic Response in van der waals materials,” Adv. Opt. Mater. Spec. Issue Polarit. Nanomater., vol. 8, p. 1901393, 2020. https://doi.org/10.1002/adom.201901393.Search in Google Scholar
 S. Dai, J. Quan, G. Hu, et al.., “Hyperbolic phonon polaritons in suspended hexagonal boron nitride,” Nano Lett., vol. 19, p. 100, 2019. https://doi.org/10.1021/acs.nanolett.8b04242.Search in Google Scholar PubMed
 S. Dai, M. Tymchenko, Z. Q. Xu, et al.., “Internal nanostructure diagnosis with hyperbolic phonon polaritons in hexagonal boron nitride,” Nano Lett., vol. 18, p. 5205, 2018. https://doi.org/10.1021/acs.nanolett.8b02162.Search in Google Scholar PubMed
 A. J. Hoffman, A. Sridhar, P. X. Braun, et al.., “Midinfrared semiconductor optical metamaterials,” J. Appl. Phys., vol. 105, p. 122411, 2009. https://doi.org/10.1063/1.3124087.Search in Google Scholar
 K. Feng, G. Harden, D. L. Sivco, and A. J. Hoffman, “Subdiffraction confinement in all-semiconductor hyperbolic metamaterial resonators,” ACS Photonics, vol. 4, p. 1621, 2017. https://doi.org/10.1021/acsphotonics.7b00309.Search in Google Scholar
 D. Lu, H. Qian, K. Wang, et al.., “Nanostructuring multilayer hyperbolic metamaterials for ultrafast and bright green InGaN quantum wells,” Adv. Mater., vol. 30, p. 15, 2018. https://doi.org/10.1002/adma.201706411.Search in Google Scholar PubMed
 I. V. Iorsh, I. S. Mukhin, I. V. Shadrivov, P. A. Belov, and Y. S. Kivshar, “Hyperbolic metamaterials based on multilayer graphene structures,” Phys. Rev. B, vol. 87, p. 075416, 2013. https://doi.org/10.1103/physrevb.87.075416.Search in Google Scholar
 E. E. Narimanov and A. V. Kildishev, “Naturally hyperbolic,” Nat. Photonics,”, vol. 9, p. 214, 2015. https://doi.org/10.1038/nphoton.2015.56.Search in Google Scholar
 G. Hu, A. Krasnok, Y. Mazor, C.-W. Qiu, and A. Alù, “Moiré hyperbolic metasurfaces,” Nano Lett., vol. 20, p. 3217, 2020. https://doi.org/10.1021/acs.nanolett.9b05319.Search in Google Scholar PubMed
 C. Wang, S. Huang, Q. Xing, et al.., “Vander Waals thin films of WTe2 for natural hyperbolic plasmonic surfaces,” Nat. Commun., vol. 11, p. 1158, 2020. https://doi.org/10.1038/s41467-020-15001-9.Search in Google Scholar PubMed PubMed Central
 E. Itai, A. J. Chaves, D. A. Rhodes, et al., “Highly confined In-plane propagating exciton-polaritons on monolayer semiconductors,” 2D Mater., vol. 7, p. 3, 2020.10.1088/2053-1583/ab8dd4Search in Google Scholar
 N. Riveraa, G. Rosolen, J. D. Joannopoulosa, I. Kaminera, and M. Soljacic, “Making two-photon processes dominate one-photon processes using mid-IR phonon polaritons,” Proc. Natl. Acad. Sci. U.S.A., vol. 114, p. 3607, 2017. https://doi.org/10.1073/pnas.1713538114.Search in Google Scholar PubMed PubMed Central
 P. A. Belov and Y. Hao, “Subwavelength imaging at optical frequencies using a transmission device formed by a periodic layered metal-dielectric structure operating in the canalization regime,” Phys. Rev. B, vol. 73, p. 113110, 2006. https://doi.org/10.1103/physrevb.73.113110.Search in Google Scholar
 P. Li, G. Hu, I. Dolado, et al.., “Collective near-field coupling and nonlocal phenomena in infrared-phononic metasurfaces for nano-light canalization,” Nat. Commun., vol. 11, p. 3663, 2020. https://doi.org/10.1038/s41467-020-17425-9.Search in Google Scholar PubMed PubMed Central
 S. Dai, Q. Ma, T. Andersen, et al.., “Subdiffractional focusing and guiding of polaritonic rays in a natural hyperbolic material,” Nat. Commun., vol. 6, p. 6963, 2015. https://doi.org/10.1038/ncomms7963.Search in Google Scholar PubMed PubMed Central
 D. Correas-Serrano, A. Alù, and J. Sebastian Gomez-Diaz, “Plasmon canalization and tunneling over anisotropic metasurfaces,” Phys. Rev. B, vol. 96, p. 075436, 2017. https://doi.org/10.1103/physrevb.96.075436.Search in Google Scholar
 P. Li, M. Lewin, A. V. Kretinin, et al.., “Hyperbolic phonon-polaritons in boron nitride for near-field optical imaging and focusing,” Nat. Commun., vol. 6, p. 7507, 2015. https://doi.org/10.1038/ncomms8507.Search in Google Scholar PubMed PubMed Central
 I.-H. Lee, M. He, X. Zhang, et al.., “Image polaritons in boron nitride for extreme polariton confinement with low losses,” Nat. Commun., vol. 11, p. 3649, 2020. https://doi.org/10.1038/s41467-020-17424-w.Search in Google Scholar PubMed PubMed Central
 A. Stahl, “Polariton Structure of interband Transitions in semiconductors,” Phys. Stat. Sol.(b), vol. 94, p.221, 1979. https://doi.org/10.1002/pssb.2220940125.Search in Google Scholar
 A. Tomadin, F. Guinea, and M. Polini, “Generation and morphing of plasmons in graphene superlattices,” Phys. Rev. B, vol. 90, p. 161406, 2014. https://doi.org/10.1103/physrevb.90.161406.Search in Google Scholar
 G. X. Ni, H. Wang, J. S. Wu, et al.., “Plasmons in graphene moiré superlattices,” Nat. Mater., vol. 14, p. 1217, 2015. https://doi.org/10.1038/nmat4425.Search in Google Scholar PubMed
 N. C. H. Hesp, I. Torre, D. R-Legrian, et al., “Collective excitations in twisted bilayer graphene close to the magic angle,” arXiv:1910.07893, 2019.Search in Google Scholar
 P. Novelli, I. Torre, F. H. L. Koppens, F. Taddei, and M. Polini, “Optical and plasmonic properties of twisted bilayer graphene: Impact of interlayer tunneling asymmetry and ground-state charge inhomogeneity,” arXiv:2005.09529, 2020.10.1103/PhysRevB.102.125403Search in Google Scholar
 D. N. Basov, R. Liang, D. A. Bonn, et al.., “In-plane anisotropy of the penetration depth in YBa2Cu3O7–x and YBa2Cu4O8 superconductors,” Phys. Rev. Lett., vol. 74, p. 598, 1995. https://doi.org/10.1103/physrevlett.74.598.Search in Google Scholar PubMed
 P. A. Wolff, “Plasma-wave instability in narrow-gap semiconductors,” Phys. Rev. Lett., vol. 24, p. 266, 1970. https://doi.org/10.1103/physrevlett.24.266.Search in Google Scholar
 T. Low, P.-Y. Chen, and D. N. Basov “Superluminal plasmons with resonant gain in population inverted bilayer graphene” Phys. Rev. B, vol. 98, p. 041403(R), 2018. https://doi.org/10.1103/physrevb.98.041403.Search in Google Scholar
 D. Dini, R. Kohler, A. Tredicucci, G. Biasiol, and L. Sorba, “Microcavity polariton splitting of intersubband transitions,” Phys. Rev. Lett., vol. 90, p. 116401, 2003. https://doi.org/10.1103/physrevlett.90.116401.Search in Google Scholar
 D. Ballarini and S. D. Liberato, “Polaritonics: from microcavities to sub-wavelength confinement,” Nanophotonics, vol. 8, p. 641, 2019. https://doi.org/10.1515/nanoph-2018-0188.Search in Google Scholar
 J. Lee, M. Tymchenko, C. Argyropoulos, et al.., “Giant nonlinear response from plasmonic metasurfaces Coupled to intersubband transitions,” Nature, vol. 511, p. 65, 2014. https://doi.org/10.1038/nature13455.Search in Google Scholar PubMed
 Y. Laplace, S. Fernandez-Pena, S. Gariglio, J. M. Triscone, and A. Cavalleri, “Proposed cavity Josephson plasmonics with complex-oxide heterostructures,” Phys. Rev. B, vol. 93, p. 075152, 2016. https://doi.org/10.1103/physrevb.93.075152.Search in Google Scholar
 D. N. Basov and T. Timusk, “Electrodynamics of high-Tc superconductors,” Rev. Mod. Phys., vol. 77, p. 721, 2005. https://doi.org/10.1103/revmodphys.77.721.Search in Google Scholar
 S. Rajasekaran, E. Casandruc, Y. Laplace, et al.., “Parametric amplification of a superconducting plasma wave,” Nat. Phys., vol. 12, p. 1012, 2016. https://doi.org/10.1038/nphys3819.Search in Google Scholar PubMed PubMed Central
 A. Charnukha, A. Sternbach, H. T. Stinson, et al.., “Ultrafast nonlocal collective dynamics of Kane plasmon-polaritons in a narrow-gap semiconductor,” Sci. Adv., vol. 5, p. eaau9956, 2019. https://doi.org/10.1126/sciadv.aau9956.Search in Google Scholar PubMed PubMed Central
 X. Li, M. Bamba, Q. Zhang, et al.., “Vacuum Bloch–Siegert shift in Landau polaritons with ultra-high cooperativity,” Nat. Photonics, vol. 12, p. 324, 2018. https://doi.org/10.1038/s41566-018-0153-0.Search in Google Scholar
 G. L. Paravicini-Bagliani, F. Appugliese, E. Richter, et al.., “Magneto-transport controlled by Landau polariton states,” Nat. Phys., vol. 15, p. 186, 2019. https://doi.org/10.1038/s41567-018-0346-y.Search in Google Scholar
 Z. Shi, X. Hong, H. A. Bechtel, et al.., “Observation of a Luttinger-liquid plasmon in metallic single-walled carbon nanotubes,” Nat. Photonics, vol. 9, p. 515, 2015. https://doi.org/10.1038/nphoton.2015.123.Search in Google Scholar
 J. M. Luttinger, “An exactly soluble model of a many-fermion system,” J. Math. Phys., vol. 4, p. 1154, 1963. https://doi.org/10.1063/1.1704046.Search in Google Scholar
 F. D. M. Haldane, “Luttinger liquid theory, of one-dimensional quantum fluids. I. Properties of the Luttinger model and their extension to the general 1D interacting spinless Fermi gas,” J. Phys. C Solid State Phys., vol. 14, p. 2585, 1981. https://doi.org/10.1088/0022-3719/14/19/010.Search in Google Scholar
 S. Wang, S. Zhao, Z. Shi, et al.., “Nonlinear Luttinger liquid plasmons in semiconducting single-walled carbon nanotubes,” Nat. Mater., vol. 19, p. 986, 2020. https://doi.org/10.1038/s41563-020-0652-5.Search in Google Scholar PubMed
 E. Camley, “Long-wavelength surface spin waves on antiferromagnets,” Phys. Rev. Lett., vol. 45, p. 283, 1980. https://doi.org/10.1103/physrevlett.45.283.Search in Google Scholar
 R. E. Camley and D. L. Millis, “Surface polaritons on uniaxial antiferromagnets,” Phys. Rev. B, vol. 26, p. 1280, 1982. https://doi.org/10.1103/physrevb.26.1280.Search in Google Scholar
 R. Macêdo and R. E. Camley, “Engineering terahertz surface magnon-polaritons in hyperbolic antiferromagnets,” Phys. Rev. B, vol. 99, p. 014437, 2019. https://doi.org/10.1103/physrevb.99.014437.Search in Google Scholar
 J. Sloan, N. Rivera, J. D. Joannopoulos, I. Kaminer, and M. Soljǎci, “Controlling spins with surface magnon polaritons,” Phys. Rev. B, vol. 100, p. 235453, 2019. https://doi.org/10.1103/physrevb.100.235453.Search in Google Scholar
 S. S. Kruk, Z. J. Wong, E. Pshenay-Severin, et al.., “Magnetic hyperbolic optical metamaterials,” Nat. Commun., vol. 7, p. 11329, 2016. https://doi.org/10.1038/ncomms11329.Search in Google Scholar PubMed PubMed Central
 P. Sivarajah, A. Steinbacher, B. Dastrup, et al.., “THz-frequency magnon-phonon-polaritons in the collective strong-coupling regime,” J. Appl. Phys., vol. 125, p. 213103, 2019. https://doi.org/10.1063/1.5083849.Search in Google Scholar
 J. J. Brion, R. F. Wallis, A. Hartstein and E. Burstein, “Theory of surface magnetoplasmons in semiconductors,” Phys. Rev. Lett., vol. 28, p. 1455, 1972.10.1103/PhysRevLett.28.1455Search in Google Scholar
 B. Hu, Y. Zhang and Q. J. Wang, “Surface magneto plasmons and their applications in the infrared frequencies,” Nanophotonics, vol. 4, p. 4, 2015. https://doi.org/10.1515/nanoph-2014-0026.Search in Google Scholar
 Z. Long, Y. Wang, M. Erukhimova, M. Tokman, and A. Belyanin, “Magnetopolaritons in Weyl semimetals in a strong magnetic field,” Phys. Rev. Lett., vol. 120, p. 037403, 2018. https://doi.org/10.1103/physrevlett.120.037403.Search in Google Scholar
 R. L. Stamps and R. E. Camley, “Focusing of magnetoplasmon polaritons,” Phys. Rev. B, vol. 31, p. 4924, 1985. https://doi.org/10.1103/physrevb.31.4924.Search in Google Scholar PubMed
 M. S. Rudner and J. C. W. Song, “Self-induced Berry flux and spontaneous non-equilibrium magnetism,” Nat. Phys., vol. 15, p. 1017, 2019. https://doi.org/10.1038/s41567-019-0578-5.Search in Google Scholar
 A. K. Geim and I. V. Grigorieva, “Van der Waals heterostructures” Nature, vol. 499, p. 419, 2013. https://doi.org/10.1038/nature12385.Search in Google Scholar PubMed
 K. S. Novoselov, A. Mishchenko, A. Carvalho and A. H. Castro Neto, “2D materials and van der Waals heterostructures” Science, vol. 353, p. 6298, 2016. https://doi.org/10.1126/science.aac9439.Search in Google Scholar PubMed
 A. Castellanos-Gomez, “Why all the fuss about 2D semiconductors?” Nat. Photonics, vol. 10, p. 202, 2016. https://doi.org/10.1038/nphoton.2016.53.Search in Google Scholar
 H. Schmidt, T. Ludtke, P. Barthold, E. McCann, V. I. Fal’ko and R. J. Haug, “Tunable graphene system with two decoupled monolayers,” Appl. Phys. Lett., vol. 93, p. 172108, 2008. https://doi.org/10.1063/1.3012369.Search in Google Scholar
 G. Li, A. Luican, J. M. B. Lopes dos Santos, et al.., “Observation of Van Hove singularities in twisted graphene layers,” Nat. Phys., vol. 6, p. 109, 2010. https://doi.org/10.1038/nphys1463.Search in Google Scholar
 J. D. Sanchez-Yamagishi, T. Taychatanapat, K. Watanabe, T. Taniguchi, A. Yacoby and P. Jarillo-Herrero, “Quantum Hall effect, screening, and layer-polarized insulating States in twisted bilayer graphene,” Phys. Rev. Lett., vol. 108, p. 076601, 2012. https://doi.org/10.1103/physrevlett.108.076601.Search in Google Scholar
 D. S. Lee, C. Riedl, T. Beringer, et al.., “Quantum Hall effect in twisted bilayer graphene" Phys. Rev. Lett., vol. 107, p. 216602, 2011. https://doi.org/10.1103/physrevlett.107.216602.Search in Google Scholar
 J. D. Sanchez-Yamagishi, J. Y. Luo, A. F. Young, et al.., “Helical edge states and fractional quantum Hall effect in a graphene electron–hole bilayer,” Nat. Nanotechnol., vol. 12, p. 118, 2017. https://doi.org/10.1038/nnano.2016.214.Search in Google Scholar PubMed
 Y. Cao, J. Y. Luo, V. Fatemi, et al.., “Superlattice-induced insulating states and valley-protected orbits in twisted bilayer graphene" Phys. Rev. Lett., vol. 117, p. 116804, 2016. https://doi.org/10.1103/physrevlett.117.116804.Search in Google Scholar PubMed
 K. Liu, L. M. Zhang, T. Cao, et al.., “Evolution of interlayer coupling in twisted molybdenum disulfide bilayers,” Nat. Commun., vol. 5, p. 4966, 2014. https://doi.org/10.1038/ncomms5966.Search in Google Scholar PubMed
 M. Barbier, P. Vasilopoulos and F. M. Peeters, “Extra Dirac points in the energy spectrum for superlattices on single-layer graphene,” Phys. Rev. B, vol. 81, p. 075438, 2010. https://doi.org/10.1103/physrevb.81.075438.Search in Google Scholar
 C. R. Woods, L. Britnell, A. Eckmann, et al.., “Commensurate-incommensurate transition in graphene on hexagonal boron nitride,” Nat. Phys., vol. 10, p. 451, 2014. https://doi.org/10.1038/nphys2954.Search in Google Scholar
 B. Hunt, J. D. Sanchez-Yamagishi, A. F. Young, et al.., “Massive Dirac fermions and hofstadter butterfly in a van der Waals heterostructure,” Science, vol. 340, p. 6139, 2013. https://doi.org/10.1126/science.1237240.Search in Google Scholar PubMed
 M. Yankowitz, J. Xue, D. Cormode, et al.., “Emergence of superlattice Dirac points in graphene on hexagonal boron nitride,” Nat. Phys., vol. 8, p. 382, 2012. https://doi.org/10.1038/nphys2272.Search in Google Scholar
 Y. Cao, V. Fatemi, S. Fang, et al.., “Unconventional superconductivity in magic-angle graphene superlattices” Nature, vol. 556, p. 43, 2018. https://doi.org/10.1038/nature26160.Search in Google Scholar PubMed
 D. M. Kennes, L. Xian, M. Claassen, and A. Rubio, “One-dimensional flat bands in twisted bilayer germanium selenide,” Nat. Commun., vol. 11, p. 1124, 2020. https://doi.org/10.1038/s41467-020-14947-0.Search in Google Scholar PubMed PubMed Central
 L. Xian, D. M. Kennes, N. Tancogne-Dejean, M. Altarelli, and A. Rubio, “Multiflat bands and strong correlations in twisted bilayer boron nitride: doping-induced correlated insulator and superconductor,” Nano Lett., vol. 19, p. 4934, 2019. https://doi.org/10.1021/acs.nanolett.9b00986.Search in Google Scholar PubMed PubMed Central
 D. M. Kennes, M. Claassen, L. Xian, A. Georges, et al.,” Moiré heterostructures: a condensed matter quantum simulator”, to appear in Nat. Phys., 2020.10.1038/s41567-020-01154-3Search in Google Scholar
 X. Chen, X. Fan, L. Li, et al.., “Moiré engineering of electronic phenomena in correlated oxides,” Nat. Phys., vol. 16, p. 631, 2020. https://doi.org/10.1038/s41567-020-0865-1.Search in Google Scholar
 K. L. Seyler, P. Rivera, H. Yu, et al.., “Signatures of moire-trapped valley excitons in MoSe2/WSe2 heterobilayers,” Nature, vol. 567, p. 66, 2019. https://doi.org/10.1038/s41586-019-0957-1.Search in Google Scholar PubMed
 Yuan, B. Zheng, J. Kuntsmann, et al.., “Twist-angle-dependent interlayer exciton diffusion in WS2–WSe2 heterobilayers,” Nat. Mater., vol. 19, p. 617, 2020. https://doi.org/10.1038/s41563-020-0670-3.Search in Google Scholar PubMed
 W. Li, X. Lu, S. Dubey, L. Devenica and A. Srivastava, “Dipolar interactions between localized interlayer excitons in van der Waals heterostructures,” Nat. Mater., vol. 19, p. 624, 2020. https://doi.org/10.1038/s41563-020-0661-4.Search in Google Scholar PubMed
 Y. Bai, L. Zhou, J. Wang, et al.., “Excitons in strain-induced one- dimensional moire potentials at transition metal dichalcogenide heterojunctions,” Nat. Mater., vol. 19, p. 1068, 2020. https://doi.org/10.1038/s41563-020-0730-8.Search in Google Scholar PubMed
 S. S. Sunku, G. X. Ni, B. Y. Jiang, et al., “Photonic crystals for nano-light in moiré graphene superlattices” Science, vol. 362, p. 1153, 2018. https://doi.org/10.1126/science.aau5144.Search in Google Scholar PubMed
 G. X. Ni, H. Wang, B.-Y. Jiang, et al., “Soliton superlattices in twisted hexagonal boron nitride,” Nat. Commun., vol. 10, p. 4360, 2019. https://doi.org/10.1038/s41467-019-12327-x.Search in Google Scholar PubMed PubMed Central
 M. Chen, X. Lin, T. H. Dinh, et al., “Configurable phonon polaritons in twisted α-MoO3,” Nat. Mater., 2020. https://doi.org/10.1038/s41563-020-0781-x.Search in Google Scholar PubMed
 G. Hu, Q. Ou, G. Si, et al.., “Topological polaritons and photonic magic angles in twisted α-MoO3 bilayers,” Nature, vol. 582, p. 209, 2020. https://doi.org/10.1038/s41586-020-2359-9.Search in Google Scholar PubMed
 F. Herrera and J. Owrutsky, “Molecular polaritons for controlling chemistry with quantum optics,” J. Chem. Phys., vol. 152, p. 100902, 2020. https://doi.org/10.1063/1.5136320.Search in Google Scholar PubMed
 J. P. Long and B. K. Simpkins, “Coherent coupling between a molecular vibration and Fabry–Perot optical cavity to give hybridized states in the strong coupling limit,” ACS Photonics, vol. 2, p. 130, 2015. https://doi.org/10.1021/ph5003347.Search in Google Scholar
 B. Xiang, R. F. Ribeiro, M. Du, et al.., “Intermolecular vibrational energy transfer enabled by microcavity strong light–matter coupling,” Science, vol. 368, p. 665, 2020. https://doi.org/10.1126/science.aba3544.Search in Google Scholar PubMed
 E. Orgiu, J. George, J. A. Hutchison, et al.., “Conductivity in organic semiconductors hybridized with the vacuum field,” Nat. Mater., vol. 14, p. 1123, 2015. https://doi.org/10.1038/nmat4392.Search in Google Scholar PubMed
 R. Chikkaraddy, B. de Nijs, F. Benz, et al.., “Single-molecule strong coupling at room temperature in plasmonic nanocavities,” Nature, vol. 535, p. 127, 2016. https://doi.org/10.1038/nature17974.Search in Google Scholar PubMed PubMed Central
 B. Xiang, R. F. Ribeiro, Y. Li, et al.., “Manipulating optical nonlinearities of molecular polaritons by delocalization,” Sci. Adv., vol. 5, p. eaax5196, 2019. https://doi.org/10.1126/sciadv.aax5196.Search in Google Scholar PubMed PubMed Central
 H. Memmi, O. Benson, S. Sadofev, and S. Kalusniak, “Strong coupling between surface plasmon polaritons and molecular vibrations,” Phys. Rev. Lett., vol. 118, p. 126802, 2017. https://doi.org/10.1103/physrevlett.118.126802.Search in Google Scholar PubMed
 L. Henriet, Z. Ristivojevic, P.P. Orth, and K. Le Hur, “Quantum dynamics of the driven and dissipative Rabi model,” Phys. Rev. A, vol. 90, p. 023820, 2014. https://doi.org/10.1103/physreva.90.023820.Search in Google Scholar
 S. Schmidt and J. Koch, “Circuit QED lattices towards quantum simulation with superconducting circuits,” Ann. Phys. (Berlin), vol. 525, p. 395, 2013. https://doi.org/10.1002/andp.201200261.Search in Google Scholar
 M. Kiffner, J. Coulthard, F. Schlawin, A. Ardavan and D. Jaksch, “Mott polaritons in cavity-coupled quantum materials,” N. J. Phys., vol. 21, p. 073066, 2019. https://doi.org/10.1088/1367-2630/ab31c7.Search in Google Scholar
 W. L. Faust and C. H. Henry, “Mixing of visible and near-resonance infrared light in GaP,” Phys. Rev. Lett., vol. 17, p. 1265, 1966. https://doi.org/10.1103/physrevlett.17.1265.Search in Google Scholar
 S. A. Holmstrom, T. Stievater, M. W. Pruessner, et al.., “Guided-mode phonon-polaritons in suspended waveguides,” Phys. Rev. B, vol. 86, p. 165120, 2012. https://doi.org/10.1103/physrevb.86.165120.Search in Google Scholar
 J. D. Caldwell, L. Lindsay, V. Giannini, et al., “Low-loss, infrared and terahertz nanophotonics using surface phonon polaritons,” Nanophotonics, vol. 4, 2015. https://doi.org/10.1515/nanoph-2014-0003.Search in Google Scholar
 S. Vassant, F. Marquier, J. J. Greffet, F. Pardo, and J. L. Pelouard, “Tailoring GaAs terahertz radiative properties with surface phonons polaritons,” Appl. Phys. Lett., vol. 97, p. 161101, 2010. https://doi.org/10.1063/1.3497645.Search in Google Scholar
 P. C. M. Planken, L. D. Noordam, T. M. Kermis, and A. Lagendijk, “Femtosecond time-resolved study of the generation and propagation of phonon polaritons in LiNbo,” Phys. Rev. B, vol. 45, p.13, 1992. https://doi.org/10.1103/physrevb.45.7106.Search in Google Scholar PubMed
 T. Feurer, N. S. Stoyanov, D. W. Ward, J. C. Vaughan, E. R. Statz, and K. A. Nelson, “Terahertz polaritonics,” Annu. Rev. Mater. Res., vol. 37, p. 317, 2007. https://doi.org/10.1146/annurev.matsci.37.052506.084327.Search in Google Scholar
 S. Kojima, N. Tsumura and M. W. Takeda, “Far-infrared phonon-polariton dispersion probed by terahertz time-domain spectroscopy,” Phys. Rev. B, vol. 67, p. 035102, 2003. https://doi.org/10.1103/physrevb.67.035102.Search in Google Scholar
 H. J. Bakker, S. Hunsche, and H. Kurz, “Coherent phonon polaritons as probes of anharmonic phonons in ferroelectrics,” Rev. Mod. Phys., vol. 70, p. 2, 1998. https://doi.org/10.1103/revmodphys.70.523.Search in Google Scholar
 K.-L. Yeh, M. C. Hoffman, J. Hebling, and K. A. Nelson, “Generation of 10 μJ ultrashort terahertz pulses by optical rectification,” Appl. Phys. Lett., vol. 90, p. 171121, 2007. https://doi.org/10.1063/1.2734374.Search in Google Scholar
 A. J. Huber, N. Ocelic, and R. Hillenbrand, “Local excitation and interference of surface phonon polaritons studied by near-field infrared microscopy,” J. Microsc., vol. 229, p. 389, 2008. https://doi.org/10.1111/j.1365-2818.2008.01917.x.Search in Google Scholar PubMed
 A. J. Huber, R. Hillenbrand, B. Deutsch, and L. Novotny, “Focusing of surface phonon polaritons,” Appl. Phys. Lett., vol. 92, p. 203104, 2008. https://doi.org/10.1063/1.2930681.Search in Google Scholar
 A. A. Goyyadinov, A. Konecna, A. Chuvilin, et al., “Probing low-energy hyperbolic polaritons in van der Waals crystals with an electron microscope,” Nat. Commun., vol. 8, p. 95, 2017.10.1038/s41467-017-00056-ySearch in Google Scholar PubMed PubMed Central
 D.-Z. A. Chen, A. Narayanaswamy, and G. Chen, “Surface phonon-polariton mediated thermal conductivity enhancement of amorphous thin films,” Phys. Rev. B, vol. 72, p. 155435, 2005. https://doi.org/10.1103/physrevb.72.155435.Search in Google Scholar
 P. S. Venkataram, J. Hermann, A. Tkatchenko, and A. W. Rodriguez, “Phonon-polariton mediated thermal radiation and heat transfer among molecules and macroscopic bodies: nonlocal electromagnetic response at mesoscopic scales,” Phys. Rev. Lett., vol. 121, p. 045901, 2018. https://doi.org/10.1103/physrevlett.121.045901.Search in Google Scholar
 D. G. Cahill, P. V. Braun, G. Chen, et al.., “Nanoscale thermal transport,” Appl. Phys. Rev., vol. 1, p. 011305, 2014. https://doi.org/10.1063/1.4832615.Search in Google Scholar
 K. Kim, B. Song, V. Fernández-Hurtado, et al.., “Radiative heat transfer in the extreme near field,” Nature, vol. 528, p. 387, 2015. https://doi.org/10.1038/nature16070.Search in Google Scholar PubMed
 D. Thompson, L. Zhu, R. Mittapally, et al.., “Hundred-fold enhancement in far-field radiative heat transfer over the blackbody limit,” Nature, vol. 561, p. 216, 2018. https://doi.org/10.1038/s41586-018-0480-9.Search in Google Scholar PubMed
 Z. Zheng, J. Chen, Y. Wang, et al.., “Highly confined and tunable hyperbolic phonon Polaritons in van der waals semiconducting transition metal oxides,” Adv. Mater., vol. 30, p. 1705318, 2018. https://doi.org/10.1002/adma.201705318.Search in Google Scholar PubMed
 W. Ma, P. Alonso-Gonzalez, S. Li, et al.., “In-plane anisotropic and ultra-low-loss polaritons in a natural van der Waals crystal,” Nature, vol. 562, p. 557, 2018. https://doi.org/10.1038/s41586-018-0618-9.Search in Google Scholar PubMed
 Z. Zheng, N. Xu, S. L. Oscurato, et al.., “A mid-infrared biaxial hyperbolic van der Waals crystal,” Sci. Adv., vol. 5, p. eaav8690, 2019. https://doi.org/10.1126/sciadv.aav8690.Search in Google Scholar PubMed PubMed Central
 P. Li, I. Dolado, F. J. Alfaro-Mozaz, et al.., “Infrared hyperbolic metasurface based on nanostructured van der Waals materials,” Science, vol. 359, p. 892, 2018. https://doi.org/10.1126/science.aaq1704.Search in Google Scholar PubMed
 A. Cartella, T. F. Nova, M. Fechner, R. Merlin, and A. Cavalleri, “Parametric amplification of optical phonons,” Proc. Natl. Acad. Sci. U.S.A., vol. 115, p. 12148, 2018. https://doi.org/10.1073/pnas.1809725115.Search in Google Scholar PubMed PubMed Central
 S. Dai, F. Wenjing, N. Rivera, et al.., “Phonon polaritons in monolayers of hexagonal boron nitride” Adv. Mater., vol. 31, p. 1806603, 2019. https://doi.org/10.1002/adma.201806603.Search in Google Scholar PubMed
 A. V. Zayats, I. I. Smolyaninov and A. A. Maradudin, “Nano-optics of surface plasmon polaritons,” Phys. Rep., vol. 408, p. 131, 2005. https://doi.org/10.1016/j.physrep.2004.11.001.Search in Google Scholar
 S. A. Maier, Plasmonics: Fundamentals and Applications, Berlin, Springer, 2007.10.1007/0-387-37825-1Search in Google Scholar
 D. K. Gramotney and S. I. Bozhevolnvi, “Plasmonics beyond the diffraction limit,” Nat. Photonics, vol. 4, p. 83, 2010.10.1038/nphoton.2009.282Search in Google Scholar
 H. A. Atwater and A. Polman, “Plasmonics for improved photovoltaic devices,” Nat. Mater., vol. 9, p. 205, 2010. https://doi.org/10.1038/nmat2629.Search in Google Scholar PubMed
 P. Berini and I. De Leon, “Surface plasmon-polariton amplifiers and lasers,” Nat. Photonics, vol. 6, p. 16, 2012. https://doi.org/10.1038/nphoton.2011.285.Search in Google Scholar
 S. I. Bogdanov, A. Boltasseva, and V. M. Shalev, “Overcoming quantum decoherence with plasmonics,” Science, vol. 364, p. 532, 2019. https://doi.org/10.1126/science.aax3766.Search in Google Scholar PubMed
 J. Lee, S. Jung, P. Y. Chen, et al.., “Ultrafast electrically-tunable polaritonic metasurfaces,” Adv. Opt. Mater., vol. 2, p. 1057, 2014. https://doi.org/10.1002/adom.201400185.Search in Google Scholar
 M. Kauranen and A. V. Zayats, “Nonlinear plasmonics,” Nat. Photonics, vol. 6, p. 73, 2012. https://doi.org/10.1038/nphoton.2012.244.Search in Google Scholar
 J. Lee, N. Nookala, J. S. Gomez-Diaz, et al., “Ultrathin gradient nonlinear metasurfaces with giant nonlinear response,” Optica, vol. 3, p. 283, 2016.10.1364/OPTICA.3.000283Search in Google Scholar
 M. Tymchenko, J. S. Gomez-Diaz, J. Lee, M. A. Belkin, and A. Alù, “Gradient nonlinear Pancharatnam–Berry metasurfaces,” Phys. Rev. Lett., vol. 115, p. 207403, 2015. https://doi.org/10.1103/physrevlett.115.207403.Search in Google Scholar
 Z. Jacob, and V. M. Shalev, “Plasmonics goes quantum,” Science, vol. 334, p. 463, 2011. https://doi.org/10.1126/science.1211736.Search in Google Scholar PubMed
 M. S. Tame, K. R. McEnery, S. K. Ozdemir, J. Lee, S. A. Maier, and M. S. Kim, “Quantum plasmonics,” Nat. Phys., vol. 9, p. 329, 2013. https://doi.org/10.1038/nphys2615.Search in Google Scholar
 S. I. Bozhevolnvi and J. B. Khurgin, “The case for quantum plasmonics,” Nat. Photonics, vol. 11, p. 398, 2017.10.1038/nphoton.2017.103Search in Google Scholar
 J. S. Fakonas, A. Mitskovets, and H. A. Atwater, “Path entanglement of surface plasmons,” New J. Phys., vol. 17, p. 023002, 2015. https://doi.org/10.1088/1367-2630/17/2/023002.Search in Google Scholar
 M.-C. Dheur, F. Devaux, T. W. Ebbesen, et al.., “Single-plasmon interferences,” Sci. Adv., vol. 2, p. e1501574, 2016. https://doi.org/10.1126/sciadv.1501574.Search in Google Scholar PubMed PubMed Central
 M. Wagner, A. S. McLeod, S. J. Maddox, et al.., “Ultrafast dynamics of surface plasmons in InAs by time-resolved infrared nanospectroscopy,” Nano Lett., vol. 14, p. 4529, 2014. https://doi.org/10.1021/nl501558t.Search in Google Scholar PubMed
 K. F. MacDonald, Z. L. Samson, M. I. Stockman and N. I. Zheludev, “Ultrafast active plasmonics,” Nat. Photonics, vol. 3, p. 55, 2009. https://doi.org/10.1038/nphoton.2008.249.Search in Google Scholar
 M. Eisele, T. L. Cocker, M. A. Huber, et al.., “Ultrafast multi-terahertz nano-spectroscopy with sub-cycle temporal resolution,” Nat. Photonics, vol. 8, p. 841, 2014. https://doi.org/10.1038/nphoton.2014.225.Search in Google Scholar
 M. A. Huber, F. Mooshammer, M. Plankl, et al.., “Femtosecond photo-switching of interface polaritons in black phosphorus heterostructures,” Nat. Nanotechnol., vol. 12, p. 207, 2017. https://doi.org/10.1038/nnano.2016.261.Search in Google Scholar PubMed
 Z. Yao, S. Xu, D. Hu, X. Chen, Q. Dai, and M. Liu, “Nanoimaging and nanospectroscopy of polaritons with time resolved s-SNOM,” Adv. Opt. Mater., vol. 8, p. 1901042, 2020. https://doi.org/10.1002/adom.201901042.Search in Google Scholar
 A V Krasavin, A. V. Zayats and N. I. Zheludev, “Active control of surface plasmon-polariton waves,” J. Opt. Pure Appl. Opt., vol. 7, p. S85, 2005. https://doi.org/10.1088/1464-4258/7/2/011.Search in Google Scholar
 J. Shi, M. H. Lin, I. T. Chen, et al.., “Cascaded exciton energy transfer in a monolayer semiconductor lateral heterostructure assisted by surface plasmon polariton,” Nat. Commun., vol. 8, p. 35, 2017. https://doi.org/10.1038/s41467-017-00048-y.Search in Google Scholar PubMed PubMed Central
 B. Min, E. Ostby, V. Sorger, et al.., “High-Q surface-plasmon-polariton whispering-gallery microcavity,” Nature, vol. 457, p. 455, 2009. https://doi.org/10.1038/nature07627.Search in Google Scholar PubMed
 A. Boltasseva and H. A. Atwater, “Low-loss plasmonic metamaterials,” Science, vol. 331, p. 290, 2011. https://doi.org/10.1126/science.1198258.Search in Google Scholar PubMed
 G. V. Naik and V. M. Shalaev, “Alternative plasmonic materials: beyond gold and silver,” Adv. Mater., vol. 25, p. 3264, 2013. https://doi.org/10.1002/adma.201205076.Search in Google Scholar PubMed
 F. Xia, H. Wang, D. Xiao, M. Dubey, and A. Ramasubramaniam, “Two-dimensional material nanophotonics,” Nat. Photonics, vol. 8, p. 899, 2014. https://doi.org/10.1038/nphoton.2014.271.Search in Google Scholar
 F. H. da Jornada, L. Xian, A. Rubio, and S. G. Louie, “Universal slow plasmons and giant field enhancement in atomically thin quasi-twodimensional metals,” Nat. Commun., vol. 11, p. 1013, 2020. https://doi.org/10.1038/s41467-020-14826-8.Search in Google Scholar PubMed PubMed Central
 E. H. Hwang and S. Das Sarma, “Plasmon modes of spatially separated doublelayer graphene,” Phys. Rev. B, vol. 80, p. 205405, 2009. https://doi.org/10.1103/physrevb.80.205405.Search in Google Scholar
 A. Principi, R. Asgari, and M. Polini, “Acoustic plasmons and composite hole-acoustic plasmon satellite bands in graphene on a metal gate,” Solid State Commun., vol. 151, p. 1627, 2011. https://doi.org/10.1016/j.ssc.2011.07.015.Search in Google Scholar
 R. E. V. Profumo, R. Asgari, M. Polini, and A. H. MacDonald, “Double-layer graphene and topological insulator thin-film plasmons,” Phys. Rev. B, vol. 85, p. 085443, 2012. https://doi.org/10.1103/physrevb.85.085443.Search in Google Scholar
 S. Chen, M. Autore, J. Li, P. Li, et al.., “Acoustic graphene plasmon nanoresonators for field-enhanced infrared molecular spectroscopy,” ACS Photonics, vol. 4, p. 3089, 2017. https://doi.org/10.1021/acsphotonics.7b00654.Search in Google Scholar
 T. Stauber and G. Gomez-Santos, “Plasmons in layered structures including graphene,” New J. Phys., vol. 14, p. 105018, 2012. https://doi.org/10.1088/1367-2630/14/10/105018.Search in Google Scholar
 I.-H. Lee, D. Yoo, P. Avouris, T. Low and S.-H. Oh, “Graphene acoustic plasmon resonator for ultrasensitive infrared spectroscopy, “Nat. Nanotechnol., vol. 14, p. 313, 2019. https://doi.org/10.1038/s41565-019-0363-8.Search in Google Scholar PubMed
 P. Alonso-Gonzalez, A. Y. Nikitin, Y. Gao, et al.., “Acoustic terahertz graphene plasmons revealed by photocurrent nanoscopy,” Nat. Nanotechnol., vol. 12, p. 31, 2017. https://doi.org/10.1038/nnano.2016.185.Search in Google Scholar PubMed
 M. B. Lundeberg, Y. Gao, R. Asgari, et al.., “Tuning quantum nonlocal effects in graphene plasmonics,” Science, vol. 347, p. 187, 2017. https://doi.org/10.1126/science.aan2735.Search in Google Scholar PubMed
 J. B. Pendry, L. Martin-Moreno, and F. J. Garcia-Vidal, “Mimicking surface plasmons with structured surfaces,” Science, vol. 305, p. 847, 2014.10.1126/science.1098999Search in Google Scholar PubMed
 M. V. Berry and N. L. Balazs, “Nonspreading wave packets,” Am. J. Phys., vol. 47, p. 264, 1979. https://doi.org/10.1119/1.11855.Search in Google Scholar
 A. Minovich, A. E. Klein, N. Janunts, T. Pertsch, D. N. Neshev, and Y. S. Kivshar, “Generation and near-field Imaging of airy surface plasmons,” Phys. Rev. Lett., vol. 107, p. 116802, 2011. https://doi.org/10.1103/physrevlett.107.116802.Search in Google Scholar
 M. Hentschel, M. Schäferling, X. Duan, H. Giessen, N. Liu, “Chiral plasmonics,” Sci. Adv., vol. 3, p. e1602735, 2017. https://doi.org/10.1126/sciadv.1602735.Search in Google Scholar PubMed PubMed Central
 T. Stauber, T. Low, and G. Gómez-Santos, “Chiral response of twisted bilayer graphene,”Phys. Rev. Lett., vol. 120, p. 046801, 2018. https://doi.org/10.1103/physrevlett.120.046801.Search in Google Scholar PubMed
 D. N. Basov and M. M. Fogler, “Quantum Materials: The quest for ultrafast plasmonics,” Nat. Nanotechnol., vol. 12, p. 187, 2017. https://doi.org/10.1038/nnano.2016.283.Search in Google Scholar PubMed
 P. Vasa, W. Wang, R. Pomraenke, et al.., “Real-time observation of ultrafast Rabi oscillations between excitons and plasmons in metal nanostructures with J-aggregates,” Nat. Photonics, vol. 7, p. 128, 2013. https://doi.org/10.1038/nphoton.2012.340.Search in Google Scholar
 N. T. Fofang, T. H. Park, O. Neumann, N. A. Mirin, P. Nordlander and N. J. Halas, “Plexcitonic nanoparticles: plasmon-exciton coupling in nanoshell-J-aggregate complexes,” Nano Lett., vol. 8, p. 3481, 2008. https://doi.org/10.1021/nl8024278.Search in Google Scholar PubMed
 N. T. Fofang, N. K. Grady, Z. Fan, A. O. Govorov, and N. J. Halas, “Plexciton dynamics: exciton-plasmon coupling in a J-aggregate–Au nanoshell complex provides a mechanism for nonlinearity,” Nano Lett., vol. 11, p. 1556, 2011. https://doi.org/10.1021/nl104352j.Search in Google Scholar PubMed
 A. Manjavacas, F. J. Garcia de Abajo and P. Nordlander, “Quantum plexcitonics: strongly interacting plasmons and excitons,” Nano Lett., vol. 11, p. 2318, 2011. https://doi.org/10.1021/nl200579f.Search in Google Scholar PubMed
 J. Yuen-Zhou, S. K. Saikin, T. Zhu, et al.., “Plexciton Dirac points and topological modes,” Nat. Commun., vol. 7, p. 11783, 2016. https://doi.org/10.1038/ncomms11783.Search in Google Scholar PubMed PubMed Central
 A. P. Manuel, A. Kirkey, N. Mahdi and K. Shankar, “Plexcitonics – fundamental principles and optoelectronic applications,” J. Mater. Chem. C, vol. 7, 2019. https://doi.org/10.1039/c8tc05054f.Search in Google Scholar
 K. Wu, W. E. Rodriguez-Cordoba, Y. Yang, and T. Lian, “Plasmon-induced hot electron transfer from the Au tip to CdS rod in CdS-Au nanoheterostructures,” Nano Lett., vol. 13, p. 5255, 2013. https://doi.org/10.1021/nl402730m.Search in Google Scholar PubMed
 P. Torma and W. L. Barnes, “Strong coupling between surface plasmon polaritons and emitters: a review,” Rep. Prog. Phys., vol. 78, p. 013901, 2015. https://doi.org/10.1088/0034-4885/78/1/013901.Search in Google Scholar PubMed
 P. A. D. Goncalves, L. P. Bertelsen, S. Xiao and N. Mortensen, “Plasmon-exciton polaritons in two-dimensional semiconductor/metal interfaces,” Phys. Rev. B, vol. 97, p. 041402, 2018. https://doi.org/10.1103/physrevb.97.041402.Search in Google Scholar
 V. Karanikolas, I. Thanopulos, and E. Paspalakis, “Strong interaction of quantum emitters with a WS2 layer enhanced by a gold substrate,” Opt. Lett., vol. 44, p. 2049, 2019. https://doi.org/10.1364/ol.44.002049.Search in Google Scholar
 T. Chervy, S. Azzini, E. Lorchat, et al.., “Room temperature chiral coupling of valley excitons with spin-momentum locked surface plasmons” ACS Photonics, vol. 5, p. 1281, 2018. https://doi.org/10.1021/acsphotonics.7b01032.Search in Google Scholar
 H. Groß, J. M. Hamm, T. Tufarelli, O. Hess, and B. Hecht, “Near-field strong coupling of single quantum dots,” Sci. Adv., vol. 4, p. eaar4906, 2018. https://doi.org/10.1126/sciadv.aar4906.Search in Google Scholar PubMed PubMed Central
 M. A. May, D. Fialkow, T. Wu, et al.., “Nano-cavity QED with tunable nano-tip interaction,” Adv. Quantum Technol., vol. 3, p. 190087, 2020. https://doi.org/10.1002/qute.201900087.Search in Google Scholar
 M. Saba, C. Ciuti, J. Bloch, et al.., “High-temperature ultrafast polariton parametric amplification in semiconductor microcavities,” Nature, vol. 414, p. 731, 2001. https://doi.org/10.1038/414731a.Search in Google Scholar PubMed
 S. Kéna-Cohen and S. R. Forrest, “Room-temperature polariton lasing in an organic single-crystal microcavity,” Nat. Photonics, vol. 4, p. 371, 2010. https://doi.org/10.1038/nphoton.2010.86.Search in Google Scholar
 H. Deng, G. Weihs, D. Snoke, J. Bloch, and Y. Yamamoto, “Polariton lasing vs. photon lasing in a semiconductor microcavity,” Proc. Natl. Acad. Sci. U.S.A., vol. 23, p. 5318, 2003.10.1073/pnas.2634328100Search in Google Scholar PubMed PubMed Central
 Y. Liu, H. Fang, A. Rasmita, et al.., “Room temperature nanocavity laser with interlayer excitons in 2D heterostructures,” Sci. Adv., vol. 5, p. eaav4506, 2019. https://doi.org/10.1126/sciadv.aav4506.Search in Google Scholar PubMed PubMed Central
 J. Flick, N. Rivera and P. Narang, “Strong light–matter coupling in quantum chemistry and quantum photonics,” Nanophotonics, vol. 7, p. 1479, 2018. https://doi.org/10.1515/nanoph-2018-0067.Search in Google Scholar
 J. A. Hutchison, T. Schwartz, C. Genet, E. Devaux, and T. W. Ebbesen, “Modifying chemical landscapes by coupling to vacuum fields,” Angew. Chem. Int. Ed., vol. 51, p. 1592, 2012. https://doi.org/10.1002/anie.201107033.Search in Google Scholar PubMed
 J. Yuen-Zhou and V. M. Menon, “Polariton chemistry: thinking inside the (photon) box,” Proc. Natl. Acad. Sci. U.S.A., vol. 116, p. 5214, 2019. https://doi.org/10.1073/pnas.1900795116.Search in Google Scholar PubMed PubMed Central
 J. Flick, M. Ruggenthaler, H. Appel, and A. Rubio “Atoms and molecules in cavities: from weak to strong coupling in QED chemistry,” Proc. Natl. Acad. Sci. U.S.A., vol. 114, p. 3026, 2017. https://doi.org/10.1073/pnas.1615509114.Search in Google Scholar PubMed PubMed Central
 C. Schäfer, M. Ruggenthaler, V. Rokaj, and A. Rubio, “Relevance of the quadratic diamagnetic and self-polarization terms in cavity quantum electrodynamics,” ACS Photonics, vol. 7, p. 975, 2020. https://doi.org/10.1021/acsphotonics.9b01649.Search in Google Scholar PubMed PubMed Central
 D. Sanvitto and S. Kéna-Cohen, “The road towards polaritonic devices,” Nat. Mater., vol. 15, p. 1061, 2016. https://doi.org/10.1038/nmat4668.Search in Google Scholar PubMed
 A. Amo, T. C. H. Liew, C. Adrados, et al.., “Exciton-polariton spin switches,” Nat. Photonics, vol. 4, p. 361, 2010. https://doi.org/10.1038/nphoton.2010.79.Search in Google Scholar
 T. Gao, P. Eldridge, T. Liew, et al.., “Polariton condensate transistor switch,” Phys. Rev. B, vol. 85, p. 235102, 2012. https://doi.org/10.1103/physrevb.85.235102.Search in Google Scholar
 D. Ballarini, M. De Giorgi, E. Cancellieri, et al.., “All-optiocal polariton transistor,” Nat. Commun., vol. 4, p. 1778, 2013. https://doi.org/10.1038/ncomms2734.Search in Google Scholar PubMed
 C. Antón, T. C. H. Liew, J. Cuadra, et al.., “Quantum refelctions and shunting of polariton condensate wave trains: Implementation of a logic AND gate,” Phys. Rev. B, vol. 88, p. 245307, 2013. https://doi.org/10.1103/physrevb.88.245307.Search in Google Scholar
 H. S. Nguyen, D. Vishnevsky, C. Sturm, et al.., “Realization of a double-barrier resonant tunneling Diode for cavity polaritons,” Phys. Rev. Lett., vol. 110, p. 236601, 2013. https://doi.org/10.1103/physrevlett.110.236601.Search in Google Scholar
 F. Marsault, H. S. Nguuyen, D. Tanese, et al.., “Realization of an all optical exciton-polariton router,” Appl. Phys. Lett., vol. 107, p. 201115, 2015. https://doi.org/10.1063/1.4936158.Search in Google Scholar
 A. Kavokin, T. C. H. Liew, C. Schneider, S. Hofling “Bosonic lasers” Low Temp. Phys., vol. 42, p. 323, 2016. https://doi.org/10.1063/1.4948614.Search in Google Scholar
 D. Ballarini, A. Gianfrate, R. Panico, et al.., “Polaritonic neuromorphic computing outperforms linear classifiers,” Nano Lett., vol. 20, p. 3506, 2020. https://doi.org/10.1021/acs.nanolett.0c00435.Search in Google Scholar PubMed
 J. Gu, B. Chakraborty, M. Khatoniar and V. M. Menon, “A room-temperature polariton light-emitting diode based on monolayer WS2,” Nat. Nanotechnol., vol. 14, p. 1024, 2019. https://doi.org/10.1038/s41565-019-0543-6.Search in Google Scholar PubMed
 E. A. Cerda-Méndez, D. N. Krizhanovskii, M. Wouters, et al.., “Polariton Condensation in dynamic acoustic lattices,” Phys. Rev. Lett., vol. 105, p. 116402, 2010. https://doi.org/10.1103/physrevlett.105.116402.Search in Google Scholar
 A. Amo and J. Bloch, “Exciton-polaritons in lattices: a non-linear photonic simulator,” Compt. Rendus Phys., vol. 17, p. 934, 2016. https://doi.org/10.1016/j.crhy.2016.08.007.Search in Google Scholar
 L. Zhang, W. Xie, J. Wang, et al.., “Weak lasing in one-dimensional polariton superlattices,” Proc. Natl. Acad. Sci. U.S.A., vol. 112, p. E1516, 2015. https://doi.org/10.1073/pnas.1502666112.Search in Google Scholar PubMed PubMed Central
 M. J. Hartmann, F. G. S. L. Brandao, and M. B. Plenio, “Quantum many-body phenomena in coupled cavity arrays,” Laser Photonics, vol. 2, p. 6, 2008. https://doi.org/10.1002/lpor.200810046.Search in Google Scholar
 N. Y. Kim and Y. Yamamoto, “Exciton-Polariton Quantum Simulators in Quantum Simulations with Photons and Polaritons,” vol. 91, D. Angelakis, ed., Springer, 2017.10.1007/978-3-319-52025-4_5Search in Google Scholar
 I. M. Georgescu, S. Ashhab and F. Nori, “Quantum simulation,” Rev. Mod. Phys., vol. 86, p. 153, 2014. https://doi.org/10.1103/revmodphys.86.153.Search in Google Scholar
 J. I. Cirac and P. Zoller, “Golas and opportunities in quantum simulation,” Nat. Phys., vol. 8, p. 264, 2012. https://doi.org/10.1038/nphys2275.Search in Google Scholar
 I. Bloch, J. Dalibard, and S. Nascimbene, “Quantum simulations with ultracold quantum gases,” Nat. Phys., vol. 8, p. 267, 2012. https://doi.org/10.1038/nphys2259.Search in Google Scholar
 N. C. Harris, G. R. Steinbrecher, M. Prabhu, et al.., “Quantum transport simulations in a programmable nanophotonic processor,” Nat. Photonics, vol. 11, p. 447, 2017. https://doi.org/10.1038/nphoton.2017.95.Search in Google Scholar
 A. Aspuru-Guzik and P. Walther, “Photonic quantum simulators,” Nat. Phys., vol. 8, p. 285, 2012. https://doi.org/10.1038/nphys2253.Search in Google Scholar
 M. J. Hartmann, F. G. S. L. Brandao, and M. B. Plenio, “Strongly interacting polaritons in coupled arrays of cavities,” Nat. Phys., vol. 2, p. 849, 2006. https://doi.org/10.1038/nphys462.Search in Google Scholar
 A. D. Greentree, C. Tahan, J. H. Cole, and L. C. L. Hollenberg, “Quantum phase transitions of light,” Nat. Phys., vol. 2, p. 856, 2006. https://doi.org/10.1038/nphys466.Search in Google Scholar
 T. Byrnes, P. Recher, and Y. Yamamoto, “Mott transitions of excitons polaritons and indirect excitons in a periodic potential,” Phys. Rev. B, vol. 81, p. 205312, 2010. https://doi.org/10.1103/physrevb.81.205312.Search in Google Scholar
 N. Na and Y. Yamamoto, “Massive parallel generation of indistinguishable single photons iva the polaritonic superfluid to Mott-insulator quantum phase transition,” New J. Phys., vol. 12, p. 123001, 2010. https://doi.org/10.1088/1367-2630/12/12/123001.Search in Google Scholar
 N. G. Berlo, M. Silva, K. Kalinin, et al., “Realizing the classical XY Hamiltonian in polariton simulators,” Nat. Mater., vol. 16, p. 1120, 2017.10.1038/nmat4971Search in Google Scholar PubMed
 T. Esslinger, “Fermi-hubbard Physics with Atoms in an optical lattice,” Ann. Rev. Condensed Matter Phys., vol. 1, p. 129, 2010. https://doi.org/10.1146/annurev-conmatphys-070909-104059.Search in Google Scholar
 R. Blatt and C. F. Roos, “Quantum simulations with trapped ions,” Nat. Phys., vol. 8, p. 277, 2012. https://doi.org/10.1038/nphys2252.Search in Google Scholar
 K. Kim, S. Korenblit, R. Islam, et al.., “Quantum simulation of the transverse Ising model with trapped ions,” New J. Phys., vol. 13, p. 105003, 2011. https://doi.org/10.1088/1367-2630/13/10/105003.Search in Google Scholar
 J. W. Britton, B. C. Sawyer, A. C. Keith, et al.., “Engineered two-dimensional Ising interactions in a trapped-ion quantum simulator with hundreds of spins,” Nature, vol. 484, p. 489, 2012. https://doi.org/10.1038/nature10981.Search in Google Scholar PubMed
 A. A. Houck, H. Tureci, and J. Koch, “On-chip quantum simulation with superconducting circuits,” Nat. Phys., vol. 8, p. 292, 2012. https://doi.org/10.1038/nphys2251.Search in Google Scholar
 J. Koch, A. A. Houck, K. Le Hur, and S. M. Girvin, “Time-reversal-symmetry breaking in circuit-QED-based photon lattices,” Phys. Rev. A, vol. 82, p. 043811, 2010. https://doi.org/10.1103/physreva.82.043811.Search in Google Scholar
 L. Xiong, C. Forsythe, M. Jung, et al., “Photonic crystal for graphene plasmons” Nat. Commun., vol. 10, p. 4780, 2019. https://doi.org/10.1038/s41467-019-12778-2.Search in Google Scholar PubMed PubMed Central
 B.-Y. Jiang, G.-X. Ni, Z. Addison, et al.., “Plasmon reflections by topological electronic boundaries in bilayer graphene,” Nano Lett., vol. 17, p. 7080, 2017. https://doi.org/10.1021/acs.nanolett.7b03816.Search in Google Scholar PubMed
 Z. Fei, G. X. Ni, B. Y. Jiang, M. M. Fogler, and D. N. Basov, “Nanoplasmonic phenomena at electronic boundaries in graphene,” ACS Photonics, vol. 4, no. 12, p. 2971, 2017. https://doi.org/10.1021/acsphotonics.7b00477.Search in Google Scholar
 J. Chen, M. L. Nesterov, A. Y. Nikitin, et al.., “Strong plasmon reflection at nanometer-size gaps in monolayer graphene on SiC,” Nano Lett., vol. 13, p. 6210, 2013. https://doi.org/10.1021/nl403622t.Search in Google Scholar PubMed
 E. H. Hasdeo and J. C. W. Song, “Long-lived domain wall plasmons in gapped bilayer graphene,” Nano Lett., vol. 17, p. 7252, 2017. https://doi.org/10.1021/acs.nanolett.7b02584.Search in Google Scholar PubMed
 R. Zia and M. L. Brongersma, “Surface plasmon polariton analogue to Young’s double-slit experiment,” Nat. Nanotechnol., vol. 2, p. 426, 2007. https://doi.org/10.1038/nnano.2007.185.Search in Google Scholar PubMed
 P. Li, M. Lewin, A. V. Kretinin, et al., “Hyperbolic phonon-polaritons in boron nitride for near-field optical imaging and focusing,” Nat. Commun., vol. 7, p. 7507, 2015.10.1038/ncomms8507Search in Google Scholar PubMed PubMed Central
 C. Yang, Q. Wu, J. Xu, K. A. Nelson, and C. A. Werley, “Experimental and theoretical analysis of THz-frequency, direction-dependent, phonon polariton modes in a subwavelength, anisotropic slab waveguide,” Opt. Express, vol. 18, p. 26351, 2010. https://doi.org/10.1364/oe.18.026351.Search in Google Scholar PubMed
 P. Peier, K. A. Nelson and T. Feurer, “Coherent phase contrast imaging of THz phonon-polariton tunneling,” Appl. Phys. B, vol. 99, p. 433, 2010. https://doi.org/10.1007/s00340-009-3886-0.Search in Google Scholar
 J. Lin, J. Dellinger, P. Genevet, B. Cluzel, F. Fornel, and F. Capasso, “Cosine-gauss plasmon beam: a localized long-range nondiffracting surface wave,” Phys. Rev. Lett., vol. 109, p. 093904, 2012. https://doi.org/10.1103/physrevlett.109.093904.Search in Google Scholar
 I. Epstein and A. Arie, “Arbitrary bending plasmonic light waves,” Phys. Rev. Lett., vol. 112, p. 023903, 2014. https://doi.org/10.1103/physrevlett.112.023903.Search in Google Scholar
 A. R. Davoyan, I. V. Shadrivov, and Y. S. Kivshar, “Self-focusing and spatial plasmon-polariton solitons,” Opt. Express, vol. 17, p. 21732, 2009. https://doi.org/10.1364/oe.17.021732.Search in Google Scholar
 J. Levinsen, G. Li, and M. M. Parish, “Microscopic description of exciton-polaritons in microcavities,” Phys. Rev. Res., vol. 1, p. 033120, 2019. https://doi.org/10.1103/physrevresearch.1.033120.Search in Google Scholar
 L. Nguyen-thˆe, S. De Liberato, M. Bamba, and C. Ciuti, “Effective polariton-polariton interactions of cavity-embedded two-dimensional electron gases,” Phys. Rev. B, vol. 87, p. 235322, 2013.10.1103/PhysRevB.87.235322Search in Google Scholar
 Y. S. Yoseob Yoon, M. Steger, G. Liu, et al., “Direct measurement of polariton–polariton interaction strength,” Nat. Phys., vol. 13, p. 870, 2017.10.1038/nphys4148Search in Google Scholar
 E. Estrecho, T. Gao, N. Bobrovska, et al., “Direct measurement of polariton-polariton interaction strength in the Thomas–Fermi regime of exciton-polariton condensation,” Phys. Rev. B, p. 035306, 2019.10.1103/PhysRevB.100.035306Search in Google Scholar
 X. Lina, Y. Yangc, N. Riverab, et al.., “All-angle negative refraction of highly squeezed plasmon and phonon polaritons in graphene–boron nitride heterostructures,” Proc. Natl. Acad. Sci. U.S.A., vol. 114, p. 6717, 2017. https://doi.org/10.1073/pnas.1701830114.Search in Google Scholar PubMed PubMed Central
 K. Chaudhary, M. Tamagnone, X. Yin, et al.., “Polariton nanophotonics using phase-change materials,” Nat. Commun., vol. 10, p. 4487, 2019. https://doi.org/10.1038/s41467-019-12439-4.Search in Google Scholar PubMed PubMed Central
 P. Alonso-González, A. Y. Nikitin, F. Golmar, et al.., “Controlling graphene plasmons with resonant metal antennas and spatial conductivity patterns,” Science, vol. 344, p. 1369, 2014. https://doi.org/10.1126/science.1253202.Search in Google Scholar PubMed
 M. Sidler, P. Back, O. Cotlet, et al.., “Fermi polaron-polaritons in charge-tunable atomically thin semiconductors,” Nat. Phys., vol. 13, p. 255, 2017. https://doi.org/10.1038/nphys3949.Search in Google Scholar
 D. K. Efimkin and A. H. MacDonald, “Many-body theory of trion absorption Features in two-dimensional semiconductors,” Phys. Rev. B, vol. 95, p. 035417, 2017. https://doi.org/10.1103/physrevb.95.035417.Search in Google Scholar
 G. Scalari, C. Maissen, D. Turcinkova, et al.., “Ultrastrong coupling of the cyclotron transition of a 2D electron gas to a THz metamaterial,” Science, vol. 335, p. 1323, 2012. https://doi.org/10.1126/science.1216022.Search in Google Scholar PubMed
 F. M. D. Pellegrino, V. Giocannetti, A. H. MacDonald, and M. Polini, “Modulated phases of graphene quantum Hall polariton fluids,” Nat. Commun., vol. 7, p. 13355, 2016. https://doi.org/10.1038/ncomms13355.Search in Google Scholar PubMed PubMed Central
 I. Neder, N. Ofek, Y. Chung, M. Heiblum, D. Mahalu, and V. Umansky, “Interference between two indistinguishable electrons from independent sources,” Nature (London), vol. 448, p. 333, 2007. https://doi.org/10.1038/nature05955.Search in Google Scholar PubMed
 C. Bäuerle, D. C. Glattli, T. Meunier, et al., “Coherent control of single electrons: a review of current progress,” Rep. Prog. Phys., vol. 81, p. 056503, 2018.10.1088/1361-6633/aaa98aSearch in Google Scholar PubMed
 J. Splettstoesser and R. J. Haug, “Single-electron control in solid state devices,” Phys. Status Solidi, vol. B254, p. 1770217, 2017. https://doi.org/10.1002/pssb.201770217.Search in Google Scholar
 D. C. Glattli and P. S. Roulleau, “Levitons for electron quantum optics,” Phys. Status Solidi, vol. B254, p. 1600650, 2016. https://doi.org/10.1002/pssb.201600650.Search in Google Scholar
 S. Smolka, W. Wuester, F. Haupt, S. Faelt, W. Wegscheider, and A. Imamoglu, “Cavity quantum electrodynamics with many-body states of a two-dimensional electron gas,” Science, vol. 346, p. 332, 2014. https://doi.org/10.1126/science.1258595.Search in Google Scholar PubMed
 P. Knuppel, S. Ravets, M. Kroner, S. Falt, W. Wegscheider, and A. Imamoglu, “Nonlinear optics in the fractional quantum Hall regime,” Nature, vol. 572, p. 91, 2019. https://doi.org/10.1038/s41586-019-1356-3.Search in Google Scholar PubMed
 L. Bing Tan, O. Cotlet, A. Bergschneider, et al.., “Interacting polaron-polaritons,” Phys. Rev. X, vol. 10, p. 021011, 2020. https://doi.org/10.1103/physrevx.10.021011.Search in Google Scholar
 M. Sich, L. E. Tapia-Rodriguez, H. Sigurdsson, et al.., “Spin domains in one-dimensional conservative polariton solitons,” ACS Photonics, vol. 5, p. 5095, 2018. https://doi.org/10.1021/acsphotonics.8b01410.Search in Google Scholar
 M. D. Lukin, M. Fleischhauer, R. Cote, et al.., “Dipole Blockade and quantum information Processing in mesoscopic atomic ensembles,” Phys. Rev. Lett., vol. 87, p. 037901, 2001. https://doi.org/10.1103/physrevlett.87.037901.Search in Google Scholar PubMed
 D. Comparat and P. Pillet, “Dipole blockade in a cold Rydberg atomic sample,” J. Opt. Soc. Am. B, vol. 27, p. A208, 2010. https://doi.org/10.1364/josab.27.00a208.Search in Google Scholar
 A. V. Gorshkov, J. Otterbach, M. Fleischhauer, T. Pohl, and M. D. Lukin, “Photon–photon interactions via Rydberg blockade,” Phys. Rev. Lett., vol. 107, p. 133602, 2011. https://doi.org/10.1103/physrevlett.107.133602.Search in Google Scholar PubMed
 E. Shahmoon, G. Kurizki, M. Fleischhauer, and D. Petrosyan, “Strongly interacting photons in hollow-core waveguides,” Phys. Rev. A, vol. 83, p. 033806, 2011. https://doi.org/10.1103/physreva.83.033806.Search in Google Scholar
 T. Peyronel, O. Firstenberg, Q.-Y. Liang, et al.., “Quantum nonlinear optics with single photons enabled by strongly interacting atoms,” Nature, vol. 488, p. 57, 2012. https://doi.org/10.1038/nature11361.Search in Google Scholar PubMed
 A. Chernikov, T. C. Berkelbach, H. M. Hill, et al.., “Exciton binding energy and nonhydrogenic Rydberg series in monolayer WS2,” Phys. Rev. Lett., vol. 113, p. 076802, 2014. https://doi.org/10.1103/physrevlett.113.076802.Search in Google Scholar
 P. Merkl, F. Mooshammer, S. Brem, et al.., “Twist-tailoring Coulomb correlations in van der Waals homobilayers,” Nat. Commun., vol. 11, p. 2167, 2020. https://doi.org/10.1038/s41467-020-16069-z.Search in Google Scholar PubMed PubMed Central
 T. Kazimierczuk, D. Fröhlich, S. Scheel, H. Stolz, and M. Bayer, “Giant Rydberg excitons in the copper oxide Cu2O,” Nature, vol. 514, p. 343, 2014. https://doi.org/10.1038/nature13832.Search in Google Scholar PubMed
 W. P. Su, J. R. Schrieffer, and A. J. Heeger, “Solitons in polyacetylene,” Phys. Rev. Lett., vol. 42, p. 1698, 1979. https://doi.org/10.1103/physrevlett.42.1698.Search in Google Scholar
 P. St-Jean, V. Goblot, E. Galopin, et al.., “Lasing in topological edge states of a one-dimensional lattice,” Nat. Photonics, vol. 11, p. 651, 2017. https://doi.org/10.1038/s41566-017-0006-2.Search in Google Scholar
 M. Bello, G. Platero, J. I. Cirac, and A. González-Tudela Bello, “Unconventional quantum optics in topological waveguide QED,” Sci. Adv., vol. 5, p. eaaw0297, 2019. https://doi.org/10.1126/sciadv.aaw0297.Search in Google Scholar PubMed PubMed Central
 C. A. Downing, T. J. Sturges, G. Weick, M. Stobinska, and L. Martin-Moreno, “Topological phases of polaritons in a cavity waveguide,” Phys. Rev. Lett., vol. 123, p. 217401, 2019. https://doi.org/10.1103/physrevlett.123.217401.Search in Google Scholar PubMed
 A. Bhattacharya, M. Zunaid Baten, I. Iorsh, T. Frost, A. Kavokin, and P. Bhattacharya, “Room-temperature spin polariton diode laser,” Phys. Rev. Lett., vol. 119, p. 067701, 2017. https://doi.org/10.1103/PhysRevLett.119.067701.Search in Google Scholar PubMed
 A. Agarwal, M. Polini, G. Vignale, and M. E. Flatt, “Long-lived spin plasmons in a spin-polarized two-dimensional electron gas,” Phys. Rev. B, vol. 90, p. 155409, 2014. https://doi.org/10.1103/physrevb.90.155409.Search in Google Scholar
 L. I. Magarill, A. V. Chaplik, and M. V. Éntin, “Spin-plasmon oscillations of the two-dimensional electron gas,” J. Exp. Theor. Phys., vol. 92, p. 15, 2001. https://doi.org/10.1134/1.1348471.Search in Google Scholar
 S. Raghu, S. Bum Chung, X. L. Qi, and S.-C. Zhang, “Collective Modes of a helical liquid,” Phys. Rev. Lett., vol. 104, p. 116401, 2010. https://doi.org/10.1103/physrevlett.104.116401.Search in Google Scholar
 J. B. Pendry, D. Schurig, and D. R. Smith, “Controlling electromagnetic electromagnetic fields,” Science, vol. 312, p. 1780, 2006. https://doi.org/10.1126/science.1125907.Search in Google Scholar PubMed
 Ulf Leonhardt, “Optical conformal mapping,” Science, vol. 312, p. 1777, 2006. https://doi.org/10.1126/science.1126493.Search in Google Scholar PubMed
 P. A. Huidobro, M. L. Nesterov, L. Martın-Moreno, and F. J. Garcıa, “Vidal transformation optics for plasmonics,” Nano Lett., vol. 10, p. 1985, 2010. https://doi.org/10.1021/nl100800c.Search in Google Scholar PubMed
 V. Ginis, P. Tassin, J. Danckaert, C. M. Soukoulis and I. Veretennicoff, “Creating electromagnetic cavities using transformation optics,” New J. Phys., vol. 14, p. 03300, 2012. https://doi.org/10.1088/1367-2630/14/3/033007.Search in Google Scholar
 A. Vakil and N. Engheta, “Transformation optics using graphene,” Science, vol. 332, p. 1291, 2011. https://doi.org/10.1126/science.1202691.Search in Google Scholar PubMed
 I. Tamm, “Über eine mögliche Art der Elektronenbindung an Kristalloberflächen,” Z. Phys., vol. 76, p. 849, 1932. https://doi.org/10.1007/bf01341581.Search in Google Scholar
 M. Kaliteevski, I. Iorsh, S. Brand, et al.., “Tamm plasmon-polaritons: possible electromagnetic states at the interface of a metal and a dielectric Bragg mirror,” Phys. Rev. B, vol. 76, p. 165415, 2007. https://doi.org/10.1103/physrevb.76.165415.Search in Google Scholar
 B. Liu, R. Wu, and V. M. Menon, “Propagating hybrid Tamm exciton Polaritons in organic microcavity,” J. Phys. Chem. C, vol. 123, no. 43, p. 26509, 2019. https://doi.org/10.1021/acs.jpcc.9b06383.Search in Google Scholar
 S. Dhara, C. Chakraborty, K. M. Goodfellow, et al.., “Anomalous dispersion of microcavity trion-polaritons,” Nat. Phys., vol. 14, p. 130, 2017. https://doi.org/10.1038/nphys4303.Search in Google Scholar
 R. P. A. Emmanuele, M. Sich, O. Kyriienko, et al.., “Highly nonlinear trion-polaritons in a monolayer semiconductor,” Nat. Commun., vol. 11, p. 3589, 2020. https://doi.org/10.1038/s41467-020-17340-z.Search in Google Scholar PubMed PubMed Central
 C. Möhl, A. Graf, F. J. Berger, et al.., “Trion-polariton formation in single-walled carbon nanotube microcavities,” ACS Photonics, vol. 5, p. 2074, 2018. https://doi.org/10.1021/acsphotonics.7b01549.Search in Google Scholar PubMed PubMed Central
 S. de Vega and F. Javier García de Abajo, “Plasmon generation through electron tunneling in graphene,” ACS Photonics, vol. 4, p. 2367, 2017. https://doi.org/10.1021/acsphotonics.7b00695.Search in Google Scholar
 A. Woessner, A. Misra, Y. Cao, et al.., “Propagating plasmons in a charge-neutral quantum tunneling transistor,” ACS Photonics, vol. 4, p. 3012, 2017. https://doi.org/10.1021/acsphotonics.7b01020.Search in Google Scholar
 X. Xu, W. Yao, D. Xiao, and T. Heinz, “Spin and pseudospins in layered transition metal dichalcogenides,” Nat. Phys., vol. 10, p. 343, 2014. https://doi.org/10.1038/nphys2942.Search in Google Scholar
 R. Peng, C. Wu, H. Li, X. Xu, and M. Li, “Separation of the valley exciton-polariton in two-dimensional semiconductors with an anisotropic photonic crystal,” Phys. Rev. B, vol. 101, p. 245418, 2020. https://doi.org/10.1103/physrevb.101.245418.Search in Google Scholar
 S. Guddala, R. Bushati, M. Li, A. B. Khanikaev, and V. M. Menon, “Valley selective optical control of excitons in 2D semiconductors using a chiral metasurface,” Opt. Mater. Express, vol. 9, p. 536, 2019. https://doi.org/10.1364/ome.9.000536.Search in Google Scholar
 I. Egri and A. Stahl, “Real space wave equation for exciton-polaritons pf wannier type,” Phys. Status Solidi, vol. 96, p. K83, 1979. https://doi.org/10.1002/pssb.2220960251.Search in Google Scholar
 G. Calajo, F. Ciccarello, D. Chang, and P. Rabl, “Atom-field dressed states in slow-light waveguide QED,” Phys. Rev. A, vol. 93, p. 033833, 2016. https://doi.org/10.1103/physreva.93.069905.Search in Google Scholar
 B. K. Ofori-Okai, P. Sivarajah, C. A. Werley, S. M. Teo, and K. A. Nelson, “Direct experimental visualization of waves and band structure in 2D photonic crystal slabs,” New J. Phys., vol. 16, p. 053003, 2014. https://doi.org/10.1088/1367-2630/16/5/053003.Search in Google Scholar
 A. Asenjo-Garcia, J. D. Hood, D. E. Chang, and H. J. Kimble, “Atom-light interactions in quasi-one-dimensional nanostructures: a Green’s-function perspective,” Phys. Rev. A, vol. 95, p. 033818, 2017. https://doi.org/10.1103/physreva.95.033818.Search in Google Scholar
 E. Vetsch, D. Reitz, G. Sagué, R. Schmidt, S. T. Dawkins, and A. Rauschenbeutel, “Optical interface created by laser-cooled atoms trapped in the evanescent field surrounding an optical nanofiber,” Phys. Rev. Lett., vol. 104, p. 203603, 2010. https://doi.org/10.1103/physrevlett.104.203603.Search in Google Scholar
 A. Goban, K. S. Choi, D. J. Alton, et al.., “Demonstration of a state-insensitive, compensated nanofiber trap,” Phys. Rev. Lett., vol. 109, p. 033603, 2012. https://doi.org/10.1103/physrevlett.109.033603.Search in Google Scholar
 A. Goban, C.-L. Hung, J. D. Hood, et al.., “Superradiance for atoms trapped along a photonic crystal waveguide,” Phys. Rev. Lett., vol. 115, p. 063601, 2015. https://doi.org/10.1103/physrevlett.115.063601.Search in Google Scholar PubMed
 J. D. Hood, A. Goban, A. Asenjo-Garcia, et al.., “Atom–atom interactions around the band edge of a photonic crystal waveguide,” Proc. Natl. Acad. Sci. U.S.A., vol. 113, p. 10507, 2016. https://doi.org/10.1073/pnas.1603788113.Search in Google Scholar PubMed PubMed Central
 M. Mirhosseini, E. Kim, X. Zhang, et al.., “Cavity quantum electrodynamics with atom-like mirrors,” Nature, vol. 569, p. 692, 2019. https://doi.org/10.1038/s41586-019-1196-1.Search in Google Scholar PubMed
 Y. Liu and A. A. Houck, “Quantum electrodynamics near a photonic bandgap,” Nat. Phys., vol. 13, p. 48, 2017. https://doi.org/10.1038/nphys3834.Search in Google Scholar
 T. Shi, Y.-H. Wu, A. González-Tudela, and J. I. Cirac, “Bound states in boson impurity models,” Phys. Rev. X, vol. 6, p. 021027, 2016. https://doi.org/10.1103/physrevx.6.021027.Search in Google Scholar
 J. Zenneck, “Fortplfanzung ebener elektromagnetischer Wellenlängs einer ebenen Leiterfläche,” Ann. Phys., vol. 328, p. 846, 1907. https://doi.org/10.1002/andp.19073281003.Search in Google Scholar
 K. A. Norton, “Propagation of radio waves over the surface of the earth and in the upper atmosphere,” Proc. IRE, vol. 24, p. 1367, 1936. https://doi.org/10.1109/jrproc.1936.227360.Search in Google Scholar
 A. Sommerfeld, “Uber die Ausbreitung der Wellen in derdrahtlosen Telegraphie,”Ann. Phys., vol. 333, p. 665, 1909. https://doi.org/10.1002/andp.19093330402.Search in Google Scholar
 M. Sarrazin and J.-P. Vigneron, “Light transmission assisted by Brewster–Zennek modes in chromium films carrying a subwavelength hole array,” Phys. Rev. B, vol. 71, p. 075404, 2005. https://doi.org/10.1103/physrevb.71.075404.Search in Google Scholar
 A. Shivola, J. Qi, and I. V. Lindell, “Bridging the gap between plasmonics and Zenneck waves,” IEEE Antenn. Propag. Mag., vol. 52, p. 124, 2010.10.1109/MAP.2010.5466406Search in Google Scholar
 K. A. Michalski and J. R. Mosig, “The sommerfeld halfspace problem redux: alternative field representations, Role of Zenneck and surface plasmon waves,” IEEE Trans. Antenn. Propag., vol. 63, 2015. https://doi.org/10.1109/tap.2015.2489680.Search in Google Scholar
 A. Yu Nikitin, S. G. Rodrigo, F. J. García-Vidal and L. Martín-Moreno, “In the diffraction shadow: Norton waves versus surface plasmon polaritons in the optical region,” New J. Phys., vol. 11, p. 123020, 2009. https://doi.org/10.1088/1367-2630/11/12/123020.Search in Google Scholar
 V. E. Babicheva, S. Gamage, L. Zhen, S. B. Cronin, V. S. Yakovlev, and Y. Abate, “Near-field surface waves in few-layer MoS2,” ACS Photonics, vol. 5, p. 2106, 2018. https://doi.org/10.1021/acsphotonics.7b01563.Search in Google Scholar
© 2020 D. N. Basov et al., published by De Gruyter, Berlin/Boston
This work is licensed under the Creative Commons Attribution 4.0 International License.